# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2023

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_p2_c
_database_code_depnum_ccdc_archive 'CCDC 2289968'
loop_
_audit_author_name
_audit_author_address
'Yingjie Zhang'
;Australian Nuclear Science and Technology Organisation
Australia
;
_audit_update_record             
;
2023-08-22 deposited with the CCDC.	2023-11-09 downloaded from the CCDC.
;
_audit_creation_date             2023-06-28
_audit_creation_method           
;
Olex2 1.5
(compiled 2021.12.09 svn.r5202d8cf for OlexSys, GUI svn.r6439)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Mg O15 U3'
_chemical_formula_sum            'Mg O15 U3'
_chemical_formula_weight         978.40
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        P21/n
_space_group_name_Hall           '-P 2yn'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   8.6310(17)
_cell_length_b                   28.231(6)
_cell_length_c                   10.601(2)
_cell_angle_alpha                90
_cell_angle_beta                 105.99(3)
_cell_angle_gamma                90
_cell_volume                     2483.1(9)
_cell_formula_units_Z            8
_cell_measurement_reflns_used    3703
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      24.997
_cell_measurement_theta_min      1.443
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    39.162
_exptl_absorpt_correction_T_max  0.4345
_exptl_absorpt_correction_T_min  0.3246
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2012/1 (Bruker,2012) was used for absorption correction.
wR2(int) was 0.1688 before and 0.0745 after correction.
The Ratio of minimum to maximum transmission is 0.7471.
The λ/2 correction factor is 0.0015.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    5.234
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             3264
_exptl_crystal_size_max          0.015
_exptl_crystal_size_mid          0.010
_exptl_crystal_size_min          0.005
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0680
_diffrn_reflns_av_unetI/netI     0.0491
_diffrn_reflns_Laue_measured_fraction_full 0.989
_diffrn_reflns_Laue_measured_fraction_max 0.989
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            29643
_diffrn_reflns_point_group_measured_fraction_full 0.989
_diffrn_reflns_point_group_measured_fraction_max 0.989
_diffrn_reflns_theta_full        24.997
_diffrn_reflns_theta_max         24.997
_diffrn_reflns_theta_min         1.443
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.989
_diffrn_measured_fraction_theta_max 0.989
_diffrn_radiation_type           
'silicon double crystal monochromated synchrotron'
_diffrn_source                   'Australian Synchrotron MX2'
_diffrn_measurement_device_type  'Eiger Detector'
_diffrn_measurement_method       'π  scans'
_diffrn_radiation_wavelength     0.71079
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                3703
_reflns_number_total             4328
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_data_collection       'BlueIce (McPhillips, et al., 2002)'
_computing_data_reduction        'XDS (Kabsch, 1993)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         4.069
_refine_diff_density_min         -4.784
_refine_diff_density_rms         0.538
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.125
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     169
_refine_ls_number_reflns         4328
_refine_ls_number_restraints     445
_refine_ls_R_factor_all          0.0699
_refine_ls_R_factor_gt           0.0645
_refine_ls_restrained_S_all      1.070
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+480.0718P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1583
_refine_ls_wR_factor_ref         0.1612
_refine_special_details          ?
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(O1) = Uanis(O2) = Uanis(O3) = Uanis(O4) = Uanis(O5) = Uanis(O6) =
Uanis(O7) = Uanis(O8) = Uanis(O9) = Uanis(O10) = Uanis(O11) = Uanis(O12) =
Uanis(O13) = Uanis(O14) = Uanis(O15) = Uanis(O16) = Uanis(O17) = Uanis(O18) =
Uanis(O19) = Uanis(O20) = Uanis(O21) = Uanis(O22) = Uanis(O23) = Uanis(O24) =
Uanis(O25) = Uanis(O26) = Uanis(O27) = Uanis(O28) = Uanis(O29) = Uanis(O30)
2. Rigid body (RIGU) restrains
 All non-hydrogen atoms
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.77674(10) 0.81149(3) 0.73702(8) 0.0122(2) Uani 1 1 d . . . . .
U2 U 0.56605(9) 0.68635(3) 0.55622(8) 0.0079(2) Uani 1 1 d . . . . .
U3 U 0.45355(10) 0.56115(3) 0.43299(8) 0.0089(2) Uani 1 1 d . . . . .
U4 U 0.72866(10) 0.56444(3) 0.76367(8) 0.0117(2) Uani 1 1 d . . . . .
U5 U 1.08194(10) 0.56135(3) 0.04885(8) 0.0091(2) Uani 1 1 d . . . . .
U6 U -0.05586(10) 0.68695(3) 0.94390(8) 0.0085(2) Uani 1 1 d . . . . .
Mg1 Mg 0.7957(10) 0.5627(3) 0.2680(8) 0.0124(15) Uani 1 1 d . . . . .
Mg2 Mg 0.2446(9) 0.6866(3) 0.7390(8) 0.0159(16) Uani 1 1 d . . . . .
O1 O 0.953(2) 0.8094(6) 0.6403(17) 0.0207(7) Uani 1 1 d . . . . .
O2 O 0.597(2) 0.8125(6) 0.8344(17) 0.0207(7) Uani 1 1 d . . . . .
O3 O 0.917(2) 0.7672(6) 0.8820(18) 0.0207(7) Uani 1 1 d . . . . .
O4 O 0.638(2) 0.8572(6) 0.6007(17) 0.0207(7) Uani 1 1 d . . . . .
O5 O 0.915(2) 0.8589(6) 0.8767(18) 0.0207(7) Uani 1 1 d . . . . .
O6 O 0.629(2) 0.7646(6) 0.5960(17) 0.0207(7) Uani 1 1 d . . . . .
O7 O 0.748(2) 0.6825(6) 0.4988(18) 0.0207(7) Uani 1 1 d . . . . .
O8 O 0.390(2) 0.6899(6) 0.6184(18) 0.0207(7) Uani 1 1 d . . . . .
O9 O 0.637(2) 0.5621(6) 0.3807(18) 0.0207(7) Uani 1 1 d . . . . .
O10 O 0.263(2) 0.5615(6) 0.4785(18) 0.0207(7) Uani 1 1 d . . . . .
O11 O 0.583(2) 0.6086(7) 0.6089(17) 0.0207(7) Uani 1 1 d . . . . .
O12 O 0.581(2) 0.5170(6) 0.6149(17) 0.0207(7) Uani 1 1 d . . . . .
O13 O 0.892(2) 0.5638(6) 0.6672(18) 0.0207(7) Uani 1 1 d . . . . .
O14 O 0.570(2) 0.5665(6) 0.8557(18) 0.0207(7) Uani 1 1 d . . . . .
O15 O 0.876(2) 0.5175(6) 0.9081(17) 0.0207(7) Uani 1 1 d . . . . .
O16 O 0.887(2) 0.6094(6) 0.9094(17) 0.0207(7) Uani 1 1 d . . . . .
O17 O 1.200(2) 0.5614(6) -0.0666(18) 0.0207(7) Uani 1 1 d . . . . .
O18 O 0.977(2) 0.5634(6) 0.1771(18) 0.0207(7) Uani 1 1 d . . . . .
O19 O 1.330(2) 0.5602(6) 0.2074(18) 0.0207(7) Uani 1 1 d . . . . .
O20 O -0.295(2) 0.6865(6) 0.7784(18) 0.0207(7) Uani 1 1 d . . . . .
O21 O 0.072(2) 0.6831(6) 0.8309(17) 0.0207(7) Uani 1 1 d . . . . .
O22 O -0.185(2) 0.6916(6) 1.0511(18) 0.0207(7) Uani 1 1 d . . . . .
O23 O 0.872(2) 0.4986(6) 0.3474(17) 0.0207(7) Uani 1 1 d . . . . .
O24 O 0.631(2) 0.5295(6) 0.1130(17) 0.0207(7) Uani 1 1 d . . . . .
O25 O 0.699(2) 0.6245(6) 0.1835(17) 0.0207(7) Uani 1 1 d . . . . .
O26 O 0.955(2) 0.5993(6) 0.4172(17) 0.0207(7) Uani 1 1 d . . . . .
O27 O 0.066(2) 0.7148(6) 0.5812(18) 0.0207(7) Uani 1 1 d . . . . .
O28 O 0.203(2) 0.6171(6) 0.6905(17) 0.0207(7) Uani 1 1 d . . . . .
O29 O 0.437(2) 0.6623(6) 0.8896(17) 0.0207(7) Uani 1 1 d . . . . .
O30 O 0.303(2) 0.7549(6) 0.7990(18) 0.0207(7) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 U2 3.6101(17) 4_676 ?
U1 U6 3.6032(18) 4_675 ?
U1 O1 2.055(18) . ?
U1 O2 2.090(18) . ?
U1 O3 2.087(18) . ?
U1 O4 2.057(18) . ?
U1 O5 2.105(18) . ?
U1 O6 2.136(18) . ?
U2 U3 3.8003(14) . ?
U2 U6 3.8248(13) 4_675 ?
U2 Mg2 3.797(8) . ?
U2 O3 2.341(18) 4_575 ?
U2 O5 2.365(18) 4_575 ?
U2 O6 2.287(18) . ?
U2 O7 1.835(18) . ?
U2 O8 1.816(18) . ?
U2 O11 2.261(18) . ?
U2 O20 2.330(18) 1_655 ?
U3 U3 3.7358(18) 3_666 ?
U3 U4 3.6535(17) . ?
U3 Mg1 3.825(8) . ?
U3 O5 2.334(18) 4_575 ?
U3 O9 1.815(18) . ?
U3 O10 1.841(18) . ?
U3 O11 2.317(18) . ?
U3 O12 2.305(18) . ?
U3 O12 2.264(18) 3_666 ?
U3 O19 2.335(18) 1_455 ?
U4 U5 3.6558(18) 1_556 ?
U4 O11 2.165(18) . ?
U4 O12 2.192(18) . ?
U4 O13 1.960(19) . ?
U4 O14 1.887(19) . ?
U4 O15 2.154(18) . ?
U4 O16 2.169(18) . ?
U5 U5 3.7768(18) 3_765 ?
U5 U6 3.8073(14) 1_654 ?
U5 Mg1 3.830(8) . ?
U5 O4 2.383(18) 4_675 ?
U5 O15 2.282(18) 3_766 ?
U5 O15 2.337(17) 1_554 ?
U5 O16 2.342(18) 1_554 ?
U5 O17 1.797(18) . ?
U5 O18 1.829(19) . ?
U5 O19 2.328(18) . ?
U6 Mg2 3.814(8) . ?
U6 O3 2.353(18) 1_455 ?
U6 O4 2.363(18) 4_576 ?
U6 O6 2.365(18) 4_576 ?
U6 O16 2.252(18) 1_455 ?
U6 O20 2.311(18) . ?
U6 O21 1.840(18) . ?
U6 O22 1.805(18) . ?
Mg1 O9 2.05(2) . ?
Mg1 O18 2.05(2) . ?
Mg1 O23 2.028(19) . ?
Mg1 O24 2.075(19) . ?
Mg1 O25 2.033(19) . ?
Mg1 O26 2.064(19) . ?
Mg2 O8 2.03(2) . ?
Mg2 O21 2.00(2) . ?
Mg2 O27 2.09(2) . ?
Mg2 O28 2.036(19) . ?
Mg2 O29 2.08(2) . ?
Mg2 O30 2.049(19) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
U6 U1 U2 171.53(3) 4_675 4_676 ?
O1 U1 U2 93.0(5) . 4_676 ?
O1 U1 U6 95.3(5) . 4_675 ?
O1 U1 O2 179.1(7) . . ?
O1 U1 O3 89.6(7) . . ?
O1 U1 O4 92.0(7) . . ?
O1 U1 O5 91.0(7) . . ?
O1 U1 O6 90.8(7) . . ?
O2 U1 U2 87.3(5) . 4_676 ?
O2 U1 U6 84.4(5) . 4_675 ?
O2 U1 O5 89.8(7) . . ?
O2 U1 O6 88.4(7) . . ?
O3 U1 U2 37.8(5) . 4_676 ?
O3 U1 U6 143.5(5) . 4_675 ?
O3 U1 O2 90.1(7) . . ?
O3 U1 O5 76.3(7) . . ?
O3 U1 O6 104.9(7) . . ?
O4 U1 U2 140.0(5) . 4_676 ?
O4 U1 U6 38.3(5) . 4_675 ?
O4 U1 O2 88.3(7) . . ?
O4 U1 O3 177.4(7) . . ?
O4 U1 O5 101.6(7) . . ?
O4 U1 O6 77.1(7) . . ?
O5 U1 U2 38.7(5) . 4_676 ?
O5 U1 U6 139.5(5) . 4_675 ?
O5 U1 O6 177.9(7) . . ?
O6 U1 U2 142.4(5) . 4_676 ?
O6 U1 U6 39.1(5) . 4_675 ?
U1 U2 U3 69.41(2) 4_575 . ?
U1 U2 U6 68.44(2) 4_575 4_675 ?
U1 U2 Mg2 93.68(12) 4_575 . ?
U3 U2 U6 137.77(3) . 4_675 ?
Mg2 U2 U3 91.37(12) . . ?
Mg2 U2 U6 88.85(13) . 4_675 ?
O3 U2 U1 33.1(4) 4_575 4_575 ?
O3 U2 U3 102.5(4) 4_575 . ?
O3 U2 U6 35.5(4) 4_575 4_675 ?
O3 U2 Mg2 94.6(5) 4_575 . ?
O3 U2 O5 66.8(6) 4_575 4_575 ?
O5 U2 U1 33.8(4) 4_575 4_575 ?
O5 U2 U3 35.7(4) 4_575 . ?
O5 U2 U6 102.2(4) 4_575 4_675 ?
O5 U2 Mg2 95.3(5) 4_575 . ?
O6 U2 U1 102.9(4) . 4_575 ?
O6 U2 U3 170.8(4) . . ?
O6 U2 U6 35.4(4) . 4_675 ?
O6 U2 Mg2 94.2(5) . . ?
O6 U2 O3 69.8(6) . 4_575 ?
O6 U2 O5 136.1(6) . 4_575 ?
O6 U2 O20 77.4(6) . 1_655 ?
O7 U2 U1 97.1(6) . 4_575 ?
O7 U2 U3 89.5(6) . . ?
O7 U2 U6 98.0(6) . 4_675 ?
O7 U2 Mg2 168.8(6) . . ?
O7 U2 O3 96.1(7) . 4_575 ?
O7 U2 O5 91.9(7) . 4_575 ?
O7 U2 O6 86.4(7) . . ?
O7 U2 O11 91.2(7) . . ?
O7 U2 O20 95.0(7) . 1_655 ?
O8 U2 U1 84.7(6) . 4_575 ?
O8 U2 U3 91.0(6) . . ?
O8 U2 U6 82.8(6) . 4_675 ?
O8 U2 Mg2 9.4(6) . . ?
O8 U2 O3 85.5(7) . 4_575 ?
O8 U2 O5 89.5(7) . 4_575 ?
O8 U2 O6 93.4(7) . . ?
O8 U2 O7 178.2(8) . . ?
O8 U2 O11 88.2(7) . . ?
O8 U2 O20 83.2(7) . 1_655 ?
O11 U2 U1 103.2(4) . 4_575 ?
O11 U2 U3 34.4(4) . . ?
O11 U2 U6 168.2(4) . 4_675 ?
O11 U2 Mg2 83.3(5) . . ?
O11 U2 O3 136.3(6) . 4_575 ?
O11 U2 O5 70.0(6) . 4_575 ?
O11 U2 O6 153.8(6) . . ?
O11 U2 O20 76.8(6) . 1_655 ?
O20 U2 U1 167.9(5) 1_655 4_575 ?
O20 U2 U3 111.2(4) 1_655 . ?
O20 U2 U6 109.5(4) 1_655 4_675 ?
O20 U2 Mg2 74.3(5) 1_655 . ?
O20 U2 O3 144.6(6) 1_655 4_575 ?
O20 U2 O5 146.2(6) 1_655 4_575 ?
U2 U3 Mg1 89.43(12) . . ?
U3 U3 U2 136.15(4) 3_666 . ?
U3 U3 Mg1 94.17(12) 3_666 . ?
U4 U3 U2 67.02(2) . . ?
U4 U3 U3 69.14(3) . 3_666 ?
U4 U3 Mg1 93.37(12) . . ?
O5 U3 U2 36.3(4) 4_575 . ?
O5 U3 U3 172.4(4) 4_575 3_666 ?
O5 U3 U4 103.3(4) 4_575 . ?
O5 U3 Mg1 86.9(5) 4_575 . ?
O5 U3 O19 75.9(6) 4_575 1_455 ?
O9 U3 U2 86.0(5) . . ?
O9 U3 U3 90.9(5) . 3_666 ?
O9 U3 U4 84.4(6) . . ?
O9 U3 Mg1 9.0(6) . . ?
O9 U3 O5 89.1(7) . 4_575 ?
O9 U3 O10 177.3(8) . . ?
O9 U3 O11 88.3(7) . . ?
O9 U3 O12 91.0(7) . 3_666 ?
O9 U3 O12 90.5(7) . . ?
O9 U3 O19 83.1(7) . 1_455 ?
O10 U3 U2 93.9(5) . . ?
O10 U3 U3 91.1(5) . 3_666 ?
O10 U3 U4 98.1(6) . . ?
O10 U3 Mg1 168.5(6) . . ?
O10 U3 O5 89.2(7) . 4_575 ?
O10 U3 O11 93.1(7) . . ?
O10 U3 O12 89.5(7) . 3_666 ?
O10 U3 O12 92.2(7) . . ?
O10 U3 O19 94.5(7) . 1_455 ?
O11 U3 U2 33.4(4) . . ?
O11 U3 U3 102.9(4) . 3_666 ?
O11 U3 U4 34.0(4) . . ?
O11 U3 Mg1 95.7(5) . . ?
O11 U3 O5 69.6(6) . 4_575 ?
O11 U3 O19 144.5(6) . 1_455 ?
O12 U3 U2 171.2(4) 3_666 . ?
O12 U3 U2 101.4(4) . . ?
O12 U3 U3 35.5(4) 3_666 3_666 ?
O12 U3 U3 34.8(4) . 3_666 ?
O12 U3 U4 34.6(4) . . ?
O12 U3 U4 104.5(4) 3_666 . ?
O12 U3 Mg1 98.0(5) . . ?
O12 U3 Mg1 88.8(5) 3_666 . ?
O12 U3 O5 137.6(6) . 4_575 ?
O12 U3 O5 152.1(6) 3_666 4_575 ?
O12 U3 O11 138.4(6) 3_666 . ?
O12 U3 O11 68.1(7) . . ?
O12 U3 O12 70.3(7) 3_666 . ?
O12 U3 O19 76.4(6) 3_666 1_455 ?
O12 U3 O19 145.9(6) . 1_455 ?
O19 U3 U2 111.4(4) 1_455 . ?
O19 U3 U3 111.6(4) 1_455 3_666 ?
O19 U3 U4 167.4(4) 1_455 . ?
O19 U3 Mg1 74.0(5) 1_455 . ?
U3 U4 U5 165.09(3) . 1_556 ?
O11 U4 U3 36.8(5) . . ?
O11 U4 U5 144.9(5) . 1_556 ?
O11 U4 O12 72.8(7) . . ?
O11 U4 O16 108.9(7) . . ?
O12 U4 U3 36.7(5) . . ?
O12 U4 U5 140.2(5) . 1_556 ?
O13 U4 U3 82.6(5) . . ?
O13 U4 U5 82.8(5) . 1_556 ?
O13 U4 O11 87.8(7) . . ?
O13 U4 O12 88.8(7) . . ?
O13 U4 O15 89.8(7) . . ?
O13 U4 O16 88.5(7) . . ?
O14 U4 U3 97.2(6) . . ?
O14 U4 U5 97.6(6) . 1_556 ?
O14 U4 O11 91.3(7) . . ?
O14 U4 O12 91.7(7) . . ?
O14 U4 O13 178.7(7) . . ?
O14 U4 O15 91.2(7) . . ?
O14 U4 O16 91.1(7) . . ?
O15 U4 U3 140.0(5) . . ?
O15 U4 U5 37.2(5) . 1_556 ?
O15 U4 O11 176.3(7) . . ?
O15 U4 O12 104.3(7) . . ?
O15 U4 O16 73.8(7) . . ?
O16 U4 U3 144.5(5) . . ?
O16 U4 U5 37.5(5) . 1_556 ?
O16 U4 O12 176.7(7) . . ?
U4 U5 U5 68.35(3) 1_554 3_765 ?
U4 U5 U6 67.29(2) 1_554 1_654 ?
U4 U5 Mg1 88.34(12) 1_554 . ?
U5 U5 U6 135.30(4) 3_765 1_654 ?
U5 U5 Mg1 85.43(12) 3_765 . ?
U6 U5 Mg1 88.05(12) 1_654 . ?
O4 U5 U4 103.8(4) 4_675 1_554 ?
O4 U5 U5 170.2(4) 4_675 3_765 ?
O4 U5 U6 36.5(4) 4_675 1_654 ?
O4 U5 Mg1 88.5(5) 4_675 . ?
O15 U5 U4 103.9(4) 3_766 1_554 ?
O15 U5 U4 33.9(4) 1_554 1_554 ?
O15 U5 U5 34.7(4) 1_554 3_765 ?
O15 U5 U5 35.6(4) 3_766 3_765 ?
O15 U5 U6 170.7(4) 3_766 1_654 ?
O15 U5 U6 100.7(4) 1_554 1_654 ?
O15 U5 Mg1 89.0(5) 3_766 . ?
O15 U5 Mg1 83.6(5) 1_554 . ?
O15 U5 O4 152.2(6) 3_766 4_675 ?
O15 U5 O4 136.8(6) 1_554 4_675 ?
O15 U5 O15 70.3(7) 3_766 1_554 ?
O15 U5 O16 137.6(6) 3_766 1_554 ?
O15 U5 O16 67.4(6) 1_554 1_554 ?
O15 U5 O19 77.1(6) 3_766 . ?
O16 U5 U4 34.3(4) 1_554 1_554 ?
O16 U5 U5 102.0(4) 1_554 3_765 ?
O16 U5 U6 33.3(4) 1_554 1_654 ?
O16 U5 Mg1 84.6(5) 1_554 . ?
O16 U5 O4 69.6(6) 1_554 4_675 ?
O17 U5 U4 86.4(6) . 1_554 ?
O17 U5 U5 93.1(6) . 3_765 ?
O17 U5 U6 89.5(6) . 1_654 ?
O17 U5 Mg1 174.8(6) . . ?
O17 U5 O4 92.2(7) . 4_675 ?
O17 U5 O15 92.7(7) . 3_766 ?
O17 U5 O15 92.4(7) . 1_554 ?
O17 U5 O16 90.8(7) . 1_554 ?
O17 U5 O18 174.9(8) . . ?
O17 U5 O19 84.8(7) . . ?
O18 U5 U4 98.3(6) . 1_554 ?
O18 U5 U5 90.5(5) . 3_765 ?
O18 U5 U6 90.5(5) . 1_654 ?
O18 U5 Mg1 10.0(6) . . ?
O18 U5 O4 84.8(7) . 4_675 ?
O18 U5 O15 88.1(7) . 3_766 ?
O18 U5 O15 92.7(7) . 1_554 ?
O18 U5 O16 92.0(7) . 1_554 ?
O18 U5 O19 90.4(7) . . ?
O19 U5 U4 171.3(5) . 1_554 ?
O19 U5 U5 112.6(4) . 3_765 ?
O19 U5 U6 112.0(4) . 1_654 ?
O19 U5 Mg1 100.4(5) . . ?
O19 U5 O4 76.1(6) . 4_675 ?
O19 U5 O15 147.1(6) . 1_554 ?
O19 U5 O16 145.2(6) . 1_554 ?
U1 U6 U2 68.57(2) 4_576 4_576 ?
U1 U6 U5 69.44(2) 4_576 1_456 ?
U1 U6 Mg2 89.21(12) 4_576 . ?
U5 U6 U2 137.99(3) 1_456 4_576 ?
U5 U6 Mg2 87.57(13) 1_456 . ?
Mg2 U6 U2 90.44(12) . 4_576 ?
O3 U6 U1 102.9(4) 1_455 4_576 ?
O3 U6 U2 35.3(4) 1_455 4_576 ?
O3 U6 U5 167.9(4) 1_455 1_456 ?
O3 U6 Mg2 82.9(5) 1_455 . ?
O3 U6 O4 134.6(6) 1_455 4_576 ?
O3 U6 O6 68.3(6) 1_455 4_576 ?
O4 U6 U1 32.7(4) 4_576 4_576 ?
O4 U6 U2 101.2(4) 4_576 4_576 ?
O4 U6 U5 36.8(4) 4_576 1_456 ?
O4 U6 Mg2 86.5(5) 4_576 . ?
O4 U6 O6 67.1(6) 4_576 4_576 ?
O6 U6 U1 34.7(4) 4_576 4_576 ?
O6 U6 U2 34.0(4) 4_576 4_576 ?
O6 U6 U5 104.0(4) 4_576 1_456 ?
O6 U6 Mg2 87.3(5) 4_576 . ?
O16 U6 U1 103.8(4) 1_455 4_576 ?
O16 U6 U2 171.5(4) 1_455 4_576 ?
O16 U6 U5 34.8(4) 1_455 1_456 ?
O16 U6 Mg2 93.3(5) 1_455 . ?
O16 U6 O3 152.9(6) 1_455 1_455 ?
O16 U6 O4 71.5(6) 1_455 4_576 ?
O16 U6 O6 138.5(6) 1_455 4_576 ?
O16 U6 O20 76.3(6) 1_455 . ?
O20 U6 U1 170.8(5) . 4_576 ?
O20 U6 U2 110.6(4) . 4_576 ?
O20 U6 U5 111.0(4) . 1_456 ?
O20 U6 Mg2 99.9(5) . . ?
O20 U6 O3 78.0(6) . 1_455 ?
O20 U6 O4 147.4(6) . 4_576 ?
O20 U6 O6 144.4(6) . 4_576 ?
O21 U6 U1 94.9(5) . 4_576 ?
O21 U6 U2 95.4(6) . 4_576 ?
O21 U6 U5 86.6(6) . 1_456 ?
O21 U6 Mg2 6.5(6) . . ?
O21 U6 O3 84.7(7) . 1_455 ?
O21 U6 O4 89.6(7) . 4_576 ?
O21 U6 O6 93.8(7) . 4_576 ?
O21 U6 O16 88.9(7) . 1_455 ?
O21 U6 O20 94.3(7) . . ?
O22 U6 U1 86.6(6) . 4_576 ?
O22 U6 U2 84.3(6) . 4_576 ?
O22 U6 U5 94.7(6) . 1_456 ?
O22 U6 Mg2 174.2(6) . . ?
O22 U6 O3 94.2(7) . 1_455 ?
O22 U6 O4 92.1(7) . 4_576 ?
O22 U6 O6 87.0(7) . 4_576 ?
O22 U6 O16 91.6(7) . 1_455 ?
O22 U6 O20 84.3(7) . . ?
O22 U6 O21 178.3(8) . . ?
U3 Mg1 U5 170.3(2) . . ?
O9 Mg1 U3 8.0(5) . . ?
O9 Mg1 U5 178.0(6) . . ?
O9 Mg1 O18 172.8(8) . . ?
O9 Mg1 O24 92.1(8) . . ?
O9 Mg1 O26 88.2(8) . . ?
O18 Mg1 U3 179.2(6) . . ?
O18 Mg1 U5 8.9(5) . . ?
O18 Mg1 O24 94.3(8) . . ?
O18 Mg1 O26 85.5(8) . . ?
O23 Mg1 U3 90.1(6) . . ?
O23 Mg1 U5 93.1(6) . . ?
O23 Mg1 O9 86.7(8) . . ?
O23 Mg1 O18 90.1(8) . . ?
O23 Mg1 O24 89.9(8) . . ?
O23 Mg1 O25 174.7(8) . . ?
O23 Mg1 O26 93.3(8) . . ?
O24 Mg1 U3 84.9(6) . . ?
O24 Mg1 U5 85.9(6) . . ?
O25 Mg1 U3 86.3(6) . . ?
O25 Mg1 U5 89.9(6) . . ?
O25 Mg1 O9 90.2(8) . . ?
O25 Mg1 O18 93.5(8) . . ?
O25 Mg1 O24 86.0(8) . . ?
O25 Mg1 O26 90.8(8) . . ?
O26 Mg1 U3 95.2(6) . . ?
O26 Mg1 U5 93.7(6) . . ?
O26 Mg1 O24 176.8(8) . . ?
U2 Mg2 U6 176.2(2) . . ?
O8 Mg2 U2 8.4(5) . . ?
O8 Mg2 U6 175.0(6) . . ?
O8 Mg2 O27 85.9(8) . . ?
O8 Mg2 O28 89.0(8) . . ?
O8 Mg2 O29 89.8(8) . . ?
O8 Mg2 O30 90.6(8) . . ?
O21 Mg2 U2 176.8(6) . . ?
O21 Mg2 U6 6.0(5) . . ?
O21 Mg2 O8 170.7(8) . . ?
O21 Mg2 O27 85.6(8) . . ?
O21 Mg2 O28 88.4(8) . . ?
O21 Mg2 O29 98.9(8) . . ?
O21 Mg2 O30 92.7(8) . . ?
O27 Mg2 U2 94.3(6) . . ?
O27 Mg2 U6 89.2(6) . . ?
O28 Mg2 U2 88.4(6) . . ?
O28 Mg2 U6 92.7(6) . . ?
O28 Mg2 O27 97.2(8) . . ?
O28 Mg2 O29 85.6(8) . . ?
O28 Mg2 O30 175.3(8) . . ?
O29 Mg2 U2 81.3(6) . . ?
O29 Mg2 U6 95.1(6) . . ?
O29 Mg2 O27 174.8(8) . . ?
O30 Mg2 U2 90.5(6) . . ?
O30 Mg2 U6 88.2(6) . . ?
O30 Mg2 O27 87.4(8) . . ?
O30 Mg2 O29 89.8(8) . . ?
U1 O3 U2 109.1(8) . 4_676 ?
U1 O3 U6 140.8(9) . 1_655 ?
U2 O3 U6 109.1(7) 4_676 1_655 ?
U1 O4 U5 144.0(9) . 4_576 ?
U1 O4 U6 109.0(8) . 4_675 ?
U6 O4 U5 106.7(7) 4_675 4_576 ?
U1 O5 U2 107.6(7) . 4_676 ?
U1 O5 U3 143.9(9) . 4_676 ?
U3 O5 U2 107.9(7) 4_676 4_676 ?
U1 O6 U2 142.5(9) . . ?
U1 O6 U6 106.3(7) . 4_675 ?
U2 O6 U6 110.6(7) . 4_675 ?
U2 O8 Mg2 162.2(11) . . ?
U3 O9 Mg1 163.0(11) . . ?
U2 O11 U3 112.2(7) . . ?
U4 O11 U2 136.9(8) . . ?
U4 O11 U3 109.2(8) . . ?
U3 O12 U3 109.7(7) 3_666 . ?
U4 O12 U3 140.5(8) . 3_666 ?
U4 O12 U3 108.6(8) . . ?
U4 O15 U5 140.6(8) . 3_766 ?
U4 O15 U5 108.9(7) . 1_556 ?
U5 O15 U5 109.7(7) 3_766 1_556 ?
U4 O16 U5 108.2(8) . 1_556 ?
U4 O16 U6 138.7(9) . 1_655 ?
U6 O16 U5 112.0(7) 1_655 1_556 ?
U5 O18 Mg1 161.0(11) . . ?
U5 O19 U3 144.1(9) . 1_655 ?
U6 O20 U2 150.5(9) . 1_455 ?
U6 O21 Mg2 167.6(11) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
U1 U2 O8 Mg2 162(4) 4_575 . . . ?
U1 U6 O21 Mg2 -29(5) 4_576 . . . ?
U2 U3 O9 Mg1 -112(4) . . . . ?
U2 U6 O21 Mg2 40(5) 4_576 . . . ?
U3 U2 O8 Mg2 93(3) . . . . ?
U3 U3 O9 Mg1 111(3) 3_666 . . . ?
U4 U3 O9 Mg1 -180(100) . . . . ?
U4 U5 O18 Mg1 9(3) 1_554 . . . ?
U5 U5 O18 Mg1 -60(3) 3_765 . . . ?
U5 U6 O21 Mg2 -98(5) 1_456 . . . ?
U6 U2 O8 Mg2 -129(4) 4_675 . . . ?
U6 U5 O18 Mg1 76(3) 1_654 . . . ?
O3 U2 O8 Mg2 -165(4) 4_575 . . . ?
O3 U6 O21 Mg2 73(5) 1_455 . . . ?
O4 U5 O18 Mg1 112(3) 4_675 . . . ?
O4 U6 O21 Mg2 -62(5) 4_576 . . . ?
O5 U2 O8 Mg2 128(4) 4_575 . . . ?
O5 U3 O9 Mg1 -76(4) 4_575 . . . ?
O6 U2 O8 Mg2 -96(4) . . . . ?
O6 U6 O21 Mg2 5(5) 4_576 . . . ?
O11 U2 O8 Mg2 58(4) . . . . ?
O11 U3 O9 Mg1 -146(4) . . . . ?
O12 U3 O9 Mg1 146(4) . . . . ?
O12 U3 O9 Mg1 76(4) 3_666 . . . ?
O15 U5 O18 Mg1 -25(3) 1_554 . . . ?
O15 U5 O18 Mg1 -95(3) 3_766 . . . ?
O16 U5 O18 Mg1 42(3) 1_554 . . . ?
O16 U6 O21 Mg2 -133(5) 1_455 . . . ?
O19 U3 O9 Mg1 0(3) 1_455 . . . ?
O19 U5 O18 Mg1 -172(3) . . . . ?
O20 U2 O8 Mg2 -19(3) 1_655 . . . ?
O20 U6 O21 Mg2 151(5) . . . . ?

_olex2_submission_special_instructions 'No special instructions were received'

# start Validation Reply Form
_vrf_PLAT971_p2_c                
;
PROBLEM: Check Calcd Resid. Dens.  0.90Ang From U4              4.81 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium and the 
ineffective absorption corrections.
;
_vrf_PLAT972_p2_c                
;
PROBLEM: Check Calcd Resid. Dens.  0.21Ang From O13            -5.18 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium and the 
ineffective absorption corrections.
;
_vrf_PLAT975_p2_c                
;
PROBLEM: Check Calcd Resid. Dens.  0.73Ang From O14     .       2.82 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium and the 
ineffective absorption corrections.
;
_vrf_PLAT976_p2_c                
;
PROBLEM: Check Calcd Resid. Dens.  1.00Ang From O10     .      -2.79 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium and the 
ineffective absorption corrections.
;
_vrf_PLAT196_p2_c                
;
PROBLEM: No TEMP record and _measurement_temperature .NE.        293 Degree
RESPONSE: The alert arises due to data collection at 100K.
;
# end Validation Reply Form
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_p1_a
_database_code_depnum_ccdc_archive 'CCDC 2289970'
loop_
_audit_author_name
_audit_author_address
'Yingjie Zhang'
;Australian Nuclear Science and Technology Organisation
Australia
;
_audit_update_record             
;
2023-08-22 deposited with the CCDC.	2023-11-09 downloaded from the CCDC.
;
_audit_creation_date             2023-06-28
_audit_creation_method           
;
Olex2 1.5
(compiled 2021.12.09 svn.r5202d8cf for OlexSys, GUI svn.r6439)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Mg Na2 O34 U8'
_chemical_formula_sum            'Mg Na2 O34 U8'
_chemical_formula_weight         2518.53
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   8.2140(16)
_cell_length_b                   8.3980(17)
_cell_length_c                   10.769(2)
_cell_angle_alpha                77.62(3)
_cell_angle_beta                 89.01(3)
_cell_angle_gamma                75.83(3)
_cell_volume                     703.0(3)
_cell_formula_units_Z            1
_cell_measurement_reflns_used    1820
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      24.995
_cell_measurement_theta_min      1.938
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    46.071
_exptl_absorpt_correction_T_max  0.4316
_exptl_absorpt_correction_T_min  0.2888
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2012/1 (Bruker,2012) was used for absorption correction.
wR2(int) was 0.0748 before and 0.0421 after correction.
The Ratio of minimum to maximum transmission is 0.6691.
The λ/2 correction factor is 0.0015.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    5.949
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             1042
_exptl_crystal_size_max          0.020
_exptl_crystal_size_mid          0.010
_exptl_crystal_size_min          0.004
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0388
_diffrn_reflns_av_unetI/netI     0.0336
_diffrn_reflns_Laue_measured_fraction_full 0.909
_diffrn_reflns_Laue_measured_fraction_max 0.909
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            8426
_diffrn_reflns_point_group_measured_fraction_full 0.909
_diffrn_reflns_point_group_measured_fraction_max 0.909
_diffrn_reflns_theta_full        24.995
_diffrn_reflns_theta_max         24.995
_diffrn_reflns_theta_min         1.938
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.909
_diffrn_measured_fraction_theta_max 0.909
_diffrn_radiation_type           
'silicon double crystal monochromated synchrotron'
_diffrn_source                   'Australian Synchrotron MX2'
_diffrn_measurement_device_type  'Eiger Detector'
_diffrn_measurement_method       'π  scans'
_diffrn_radiation_wavelength     0.71079
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                1820
_reflns_number_total             2247
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_data_collection       'BlueIce (McPhillips, et al., 2002)'
_computing_data_reduction        'XDS (Kabsch, 1993)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         3.429
_refine_diff_density_min         -2.808
_refine_diff_density_rms         0.537
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.019
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     205
_refine_ls_number_reflns         2247
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0548
_refine_ls_R_factor_gt           0.0424
_refine_ls_restrained_S_all      1.019
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0751P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1058
_refine_ls_wR_factor_ref         0.1144
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.17586(8) 0.12494(8) 0.92221(6) 0.0168(2) Uani 1 1 d . . . . .
U2 U 0.17057(8) 0.58705(8) 0.91937(6) 0.0167(2) Uani 1 1 d . . . . .
U3 U 0.44840(8) 0.85299(8) 0.64285(6) 0.0156(2) Uani 1 1 d . . . . .
U4 U 0.55693(8) 0.65339(8) 0.36987(6) 0.0170(2) Uani 1 1 d . . . . .
Mg1 Mg 0.000000 1.000000 0.500000 0.0170(18) Uani 1 2 d S . P . .
Na1 Na 0.8285(9) 0.4846(10) 0.7108(7) 0.0266(17) Uani 1 1 d . . . . .
O1 O 0.3132(15) 0.0172(15) 1.0593(11) 0.018(3) Uani 1 1 d . . . . .
O2 O 0.0420(15) 0.2277(16) 0.7839(12) 0.021(3) Uani 1 1 d . . . . .
O3 O 0.0628(15) -0.1088(15) 0.9162(12) 0.020(3) Uani 1 1 d . . . . .
O4 O 0.3963(17) 0.0294(16) 0.7983(12) 0.025(3) Uani 1 1 d . . . . .
O5 O 0.0814(16) 0.3510(15) 0.9944(12) 0.021(3) Uani 1 1 d . . . . .
O6 O 0.3555(16) 0.3368(16) 0.8523(12) 0.023(3) Uani 1 1 d . . . . .
O7 O 0.2842(15) 0.5487(16) 1.0705(11) 0.018(3) Uani 1 1 d . . . . .
O8 O 0.0679(15) 0.6198(14) 0.7664(11) 0.017(3) Uani 1 1 d . . . . .
O9 O 0.4026(17) 0.6694(18) 0.8286(13) 0.030(3) Uani 1 1 d . . . . .
O10 O 0.6688(16) 0.7748(16) 0.6943(12) 0.022(3) Uani 1 1 d . . . . .
O11 O 0.2239(15) 0.9234(15) 0.6046(11) 0.018(3) Uani 1 1 d . . . . .
O12 O 0.5088(16) 0.8864(15) 0.4360(11) 0.018(3) Uani 1 1 d . . . . .
O13 O 0.7776(16) 0.5933(17) 0.4339(13) 0.027(3) Uani 1 1 d . . . . .
O14 O 0.3441(15) 0.7117(16) 0.3031(12) 0.023(3) Uani 1 1 d . . . . .
O15 O 0.5335(15) 0.3915(16) 0.4253(11) 0.019(3) Uani 1 1 d . . . . .
O16 O 0.0117(15) 0.7538(15) 0.4979(10) 0.021(3) Uani 1 1 d . . . . .
O17 O -0.1205(15) 0.9874(15) 0.6763(11) 0.019(3) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 U2 3.8845(16) 2_567 ?
U1 U2 3.8639(12) . ?
U1 Na1 3.938(8) 1_455 ?
U1 O1 1.805(12) . ?
U1 O2 1.792(13) . ?
U1 O3 2.381(12) . ?
U1 O3 2.607(12) 2_557 ?
U1 O4 2.317(13) . ?
U1 O5 2.168(13) . ?
U1 O6 2.566(12) . ?
U2 U2 3.7087(17) 2_567 ?
U2 Na1 3.898(8) 2_667 ?
U2 Na1 3.989(8) 1_455 ?
U2 O3 2.483(12) 1_565 ?
U2 O5 2.263(12) . ?
U2 O5 2.243(13) 2_567 ?
U2 O6 2.509(13) . ?
U2 O7 1.817(11) . ?
U2 O8 1.800(12) . ?
U2 O9 2.314(13) . ?
U3 U3 3.7363(18) 2_676 ?
U3 U4 3.6793(13) . ?
U3 Mg1 3.8226(14) . ?
U3 Na1 3.773(8) . ?
U3 O4 2.431(12) 1_565 ?
U3 O9 2.336(14) . ?
U3 O10 1.820(13) . ?
U3 O11 1.819(12) . ?
U3 O12 2.247(12) . ?
U3 O12 2.281(12) 2_676 ?
U3 O15 2.295(12) 2_666 ?
U4 U4 3.6553(18) 2_666 ?
U4 Na1 3.800(8) 2_666 ?
U4 Na1 4.119(8) . ?
U4 O6 2.477(13) 2_666 ?
U4 O12 2.169(11) . ?
U4 O13 1.861(13) . ?
U4 O14 1.813(13) . ?
U4 O15 2.207(13) . ?
U4 O15 2.299(12) 2_666 ?
Mg1 O11 2.061(12) 2_576 ?
Mg1 O11 2.061(12) . ?
Mg1 O16 2.051(11) 2_576 ?
Mg1 O16 2.051(11) . ?
Mg1 O17 2.120(12) . ?
Mg1 O17 2.120(12) 2_576 ?
Na1 O2 2.412(15) 1_655 ?
Na1 O7 2.501(13) 2_667 ?
Na1 O8 2.634(14) 1_655 ?
Na1 O10 2.439(15) . ?
Na1 O13 2.931(16) . ?
Na1 O14 2.450(15) 2_666 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
U2 U1 U2 57.19(3) . 2_567 ?
U2 U1 Na1 61.49(11) . 1_455 ?
U2 U1 Na1 59.78(12) 2_567 1_455 ?
O1 U1 U2 99.7(4) . 2_567 ?
O1 U1 U2 100.7(4) . . ?
O1 U1 Na1 157.5(4) . 1_455 ?
O1 U1 O3 84.1(5) . 2_557 ?
O1 U1 O3 94.5(5) . . ?
O1 U1 O4 87.3(5) . . ?
O1 U1 O5 94.4(5) . . ?
O1 U1 O6 92.0(5) . . ?
O2 U1 U2 81.7(4) . 2_567 ?
O2 U1 U2 80.5(4) . . ?
O2 U1 Na1 23.9(4) . 1_455 ?
O2 U1 O1 178.5(5) . . ?
O2 U1 O3 96.7(5) . 2_557 ?
O2 U1 O3 84.7(5) . . ?
O2 U1 O4 91.5(5) . . ?
O2 U1 O5 87.0(5) . . ?
O2 U1 O6 88.3(5) . . ?
O3 U1 U2 39.1(3) 2_557 2_567 ?
O3 U1 U2 157.1(3) . . ?
O3 U1 U2 95.2(3) 2_557 . ?
O3 U1 U2 103.6(3) . 2_567 ?
O3 U1 Na1 84.1(3) 2_557 1_455 ?
O3 U1 Na1 99.2(3) . 1_455 ?
O3 U1 O3 69.3(5) . 2_557 ?
O3 U1 O6 157.1(4) . . ?
O4 U1 U2 106.4(3) . . ?
O4 U1 U2 163.0(3) . 2_567 ?
O4 U1 Na1 110.1(4) . 1_455 ?
O4 U1 O3 157.9(4) . 2_557 ?
O4 U1 O3 91.2(4) . . ?
O4 U1 O6 67.1(4) . . ?
O5 U1 U2 30.0(3) . . ?
O5 U1 U2 28.8(3) . 2_567 ?
O5 U1 Na1 63.2(3) . 1_455 ?
O5 U1 O3 132.4(4) . . ?
O5 U1 O3 65.2(4) . 2_557 ?
O5 U1 O4 135.9(5) . . ?
O5 U1 O6 68.8(5) . . ?
O6 U1 U2 96.9(3) . 2_567 ?
O6 U1 U2 39.9(3) . . ?
O6 U1 Na1 82.3(3) . 1_455 ?
O6 U1 O3 133.3(4) . 2_557 ?
U1 U2 U1 122.81(3) . 2_567 ?
U1 U2 Na1 91.60(11) 2_567 1_455 ?
U1 U2 Na1 60.79(11) 2_567 2_667 ?
U1 U2 Na1 60.17(11) . 1_455 ?
U1 U2 Na1 93.31(12) . 2_667 ?
U2 U2 U1 61.12(3) 2_567 2_567 ?
U2 U2 U1 61.68(3) 2_567 . ?
U2 U2 Na1 60.72(12) 2_567 1_455 ?
U2 U2 Na1 63.19(12) 2_567 2_667 ?
Na1 U2 Na1 123.92(11) 2_667 1_455 ?
O3 U2 U1 160.4(3) 1_565 . ?
O3 U2 U1 41.5(3) 1_565 2_567 ?
O3 U2 U2 101.3(3) 1_565 2_567 ?
O3 U2 Na1 104.0(3) 1_565 1_455 ?
O3 U2 Na1 86.6(3) 1_565 2_667 ?
O3 U2 O6 155.1(4) 1_565 . ?
O5 U2 U1 27.8(3) 2_567 2_567 ?
O5 U2 U1 94.9(3) . 2_567 ?
O5 U2 U1 28.6(3) . . ?
O5 U2 U1 95.8(3) 2_567 . ?
O5 U2 U2 34.8(3) 2_567 2_567 ?
O5 U2 U2 34.4(3) . 2_567 ?
O5 U2 Na1 72.4(3) . 2_667 ?
O5 U2 Na1 61.8(3) . 1_455 ?
O5 U2 Na1 70.6(3) 2_567 1_455 ?
O5 U2 Na1 63.8(3) 2_567 2_667 ?
O5 U2 O3 135.7(4) . 1_565 ?
O5 U2 O3 66.6(4) 2_567 1_565 ?
O5 U2 O5 69.2(5) 2_567 . ?
O5 U2 O6 68.5(4) . . ?
O5 U2 O6 136.7(4) 2_567 . ?
O5 U2 O9 140.3(5) . . ?
O5 U2 O9 150.2(5) 2_567 . ?
O6 U2 U1 41.0(3) . . ?
O6 U2 U1 163.3(3) . 2_567 ?
O6 U2 U2 102.5(3) . 2_567 ?
O6 U2 Na1 81.9(3) . 1_455 ?
O6 U2 Na1 110.5(3) . 2_667 ?
O7 U2 U1 83.6(4) . 2_567 ?
O7 U2 U1 97.4(4) . . ?
O7 U2 U2 91.0(4) . 2_567 ?
O7 U2 Na1 30.2(4) . 2_667 ?
O7 U2 Na1 149.3(4) . 1_455 ?
O7 U2 O3 92.3(5) . 1_565 ?
O7 U2 O5 93.3(5) . 2_567 ?
O7 U2 O5 88.3(5) . . ?
O7 U2 O6 94.2(5) . . ?
O7 U2 O9 85.6(5) . . ?
O8 U2 U1 99.3(4) . 2_567 ?
O8 U2 U1 81.6(4) . . ?
O8 U2 U2 91.0(4) . 2_567 ?
O8 U2 Na1 31.7(4) . 1_455 ?
O8 U2 Na1 152.4(4) . 2_667 ?
O8 U2 O3 89.5(5) . 1_565 ?
O8 U2 O5 89.6(5) . 2_567 ?
O8 U2 O5 92.0(5) . . ?
O8 U2 O6 83.2(5) . . ?
O8 U2 O7 177.0(5) . . ?
O8 U2 O9 92.3(5) . . ?
O9 U2 U1 123.2(4) . 2_567 ?
O9 U2 U1 113.9(4) . . ?
O9 U2 U2 174.0(4) . 2_567 ?
O9 U2 Na1 121.4(4) . 1_455 ?
O9 U2 Na1 114.4(4) . 2_667 ?
O9 U2 O3 83.7(4) . 1_565 ?
O9 U2 O6 72.9(5) . . ?
U3 U3 Mg1 85.04(4) 2_676 . ?
U3 U3 Na1 105.33(13) 2_676 . ?
U4 U3 U3 67.27(3) . 2_676 ?
U4 U3 Mg1 86.38(3) . . ?
U4 U3 Na1 67.10(12) . . ?
Na1 U3 Mg1 143.73(12) . . ?
O4 U3 U3 101.8(3) 1_565 2_676 ?
O4 U3 U4 168.9(3) 1_565 . ?
O4 U3 Mg1 94.8(3) 1_565 . ?
O4 U3 Na1 116.1(3) 1_565 . ?
O9 U3 U3 175.7(3) . 2_676 ?
O9 U3 U4 114.1(3) . . ?
O9 U3 Mg1 99.0(3) . . ?
O9 U3 Na1 72.2(4) . . ?
O9 U3 O4 76.7(5) . 1_565 ?
O10 U3 U3 91.6(4) . 2_676 ?
O10 U3 U4 87.2(4) . . ?
O10 U3 Mg1 173.5(4) . . ?
O10 U3 Na1 32.4(4) . . ?
O10 U3 O4 91.4(5) . 1_565 ?
O10 U3 O9 84.5(5) . . ?
O10 U3 O12 90.0(5) . 2_676 ?
O10 U3 O12 92.7(5) . . ?
O10 U3 O15 88.4(5) . 2_666 ?
O11 U3 U3 92.9(4) . 2_676 ?
O11 U3 U4 95.8(4) . . ?
O11 U3 Mg1 10.5(4) . . ?
O11 U3 Na1 146.4(4) . . ?
O11 U3 O4 86.4(5) . 1_565 ?
O11 U3 O9 91.0(5) . . ?
O11 U3 O10 175.3(5) . . ?
O11 U3 O12 93.0(5) . 2_676 ?
O11 U3 O12 91.8(5) . . ?
O11 U3 O15 91.7(5) . 2_666 ?
O12 U3 U3 34.7(3) . 2_676 ?
O12 U3 U3 34.1(3) 2_676 2_676 ?
O12 U3 U4 101.2(3) 2_676 . ?
O12 U3 U4 32.9(3) . . ?
O12 U3 Mg1 90.4(3) 2_676 . ?
O12 U3 Mg1 81.4(3) . . ?
O12 U3 Na1 88.0(3) . . ?
O12 U3 Na1 117.9(3) 2_676 . ?
O12 U3 O4 136.3(4) . 1_565 ?
O12 U3 O4 67.7(4) 2_676 1_565 ?
O12 U3 O9 147.0(5) . . ?
O12 U3 O9 143.8(4) 2_676 . ?
O12 U3 O12 68.8(5) . 2_676 ?
O12 U3 O15 69.4(4) . 2_666 ?
O12 U3 O15 138.0(4) 2_676 2_666 ?
O15 U3 U3 104.0(3) 2_666 2_676 ?
O15 U3 U4 36.8(3) 2_666 . ?
O15 U3 Mg1 87.0(3) 2_666 . ?
O15 U3 Na1 56.9(3) 2_666 . ?
O15 U3 O4 154.2(4) 2_666 1_565 ?
O15 U3 O9 77.7(5) 2_666 . ?
U3 U4 Na1 57.54(11) . . ?
U3 U4 Na1 106.23(12) . 2_666 ?
U4 U4 U3 71.69(3) 2_666 . ?
U4 U4 Na1 58.16(11) 2_666 . ?
U4 U4 Na1 67.05(12) 2_666 2_666 ?
Na1 U4 Na1 125.20(10) 2_666 . ?
O6 U4 U3 151.3(3) 2_666 . ?
O6 U4 U4 137.0(3) 2_666 2_666 ?
O6 U4 Na1 131.5(3) 2_666 . ?
O6 U4 Na1 89.2(3) 2_666 2_666 ?
O12 U4 U3 34.2(3) . . ?
O12 U4 U4 105.5(3) . 2_666 ?
O12 U4 Na1 80.4(3) . . ?
O12 U4 Na1 116.0(4) . 2_666 ?
O12 U4 O6 117.2(4) . 2_666 ?
O12 U4 O15 142.1(5) . . ?
O12 U4 O15 70.7(5) . 2_666 ?
O13 U4 U3 86.4(4) . . ?
O13 U4 U4 90.8(4) . 2_666 ?
O13 U4 Na1 39.4(4) . . ?
O13 U4 Na1 148.3(4) . 2_666 ?
O13 U4 O6 92.9(5) . 2_666 ?
O13 U4 O12 90.9(5) . . ?
O13 U4 O15 92.1(5) . . ?
O13 U4 O15 89.2(5) . 2_666 ?
O14 U4 U3 95.1(4) . . ?
O14 U4 U4 90.3(4) . 2_666 ?
O14 U4 Na1 142.1(4) . . ?
O14 U4 Na1 31.7(4) . 2_666 ?
O14 U4 O6 85.5(5) . 2_666 ?
O14 U4 O12 89.9(5) . . ?
O14 U4 O13 178.4(5) . . ?
O14 U4 O15 92.3(5) . 2_666 ?
O14 U4 O15 88.1(5) . . ?
O15 U4 U3 108.3(3) . . ?
O15 U4 U3 36.8(3) 2_666 . ?
O15 U4 U4 36.6(3) . 2_666 ?
O15 U4 U4 35.0(3) 2_666 2_666 ?
O15 U4 Na1 56.5(3) . 2_666 ?
O15 U4 Na1 49.9(3) 2_666 . ?
O15 U4 Na1 78.3(3) . . ?
O15 U4 Na1 84.8(3) 2_666 2_666 ?
O15 U4 O6 171.8(4) 2_666 2_666 ?
O15 U4 O6 100.4(4) . 2_666 ?
O15 U4 O15 71.6(5) . 2_666 ?
U3 Mg1 U3 180.0 . 2_576 ?
O11 Mg1 U3 9.2(3) . . ?
O11 Mg1 U3 170.8(3) . 2_576 ?
O11 Mg1 U3 170.8(3) 2_576 . ?
O11 Mg1 U3 9.2(3) 2_576 2_576 ?
O11 Mg1 O11 180.0(4) . 2_576 ?
O11 Mg1 O17 93.2(5) . 2_576 ?
O11 Mg1 O17 86.8(5) 2_576 2_576 ?
O11 Mg1 O17 93.2(5) 2_576 . ?
O11 Mg1 O17 86.8(5) . . ?
O16 Mg1 U3 87.8(3) . . ?
O16 Mg1 U3 92.2(3) 2_576 . ?
O16 Mg1 U3 92.2(3) . 2_576 ?
O16 Mg1 U3 87.8(3) 2_576 2_576 ?
O16 Mg1 O11 89.4(5) 2_576 2_576 ?
O16 Mg1 O11 90.6(5) 2_576 . ?
O16 Mg1 O11 90.6(5) . 2_576 ?
O16 Mg1 O11 89.4(5) . . ?
O16 Mg1 O16 180.0 . 2_576 ?
O16 Mg1 O17 93.4(5) . . ?
O16 Mg1 O17 86.6(5) . 2_576 ?
O16 Mg1 O17 93.4(5) 2_576 2_576 ?
O16 Mg1 O17 86.6(5) 2_576 . ?
O17 Mg1 U3 95.9(3) 2_576 2_576 ?
O17 Mg1 U3 84.1(3) 2_576 . ?
O17 Mg1 U3 95.9(3) . . ?
O17 Mg1 U3 84.1(3) . 2_576 ?
O17 Mg1 O17 180.0(6) 2_576 . ?
U1 Na1 U2 58.34(11) 1_655 1_655 ?
U1 Na1 U4 146.8(2) 1_655 . ?
U2 Na1 U1 59.43(11) 2_667 1_655 ?
U2 Na1 U2 56.08(11) 2_667 1_655 ?
U2 Na1 U4 148.1(2) 2_667 . ?
U2 Na1 U4 142.6(2) 1_655 . ?
U3 Na1 U1 156.5(2) . 1_655 ?
U3 Na1 U2 109.75(19) . 1_655 ?
U3 Na1 U2 97.08(18) . 2_667 ?
U3 Na1 U4 55.36(10) . . ?
U3 Na1 U4 69.10(13) . 2_666 ?
U4 Na1 U1 114.3(2) 2_666 1_655 ?
U4 Na1 U2 159.4(2) 2_666 1_655 ?
U4 Na1 U2 103.34(19) 2_666 2_667 ?
U4 Na1 U4 54.80(10) 2_666 . ?
O2 Na1 U1 17.6(3) 1_655 1_655 ?
O2 Na1 U2 75.4(4) 1_655 2_667 ?
O2 Na1 U2 72.2(3) 1_655 1_655 ?
O2 Na1 U3 169.7(4) 1_655 . ?
O2 Na1 U4 129.2(4) 1_655 . ?
O2 Na1 U4 105.3(4) 1_655 2_666 ?
O2 Na1 O7 88.8(5) 1_655 2_667 ?
O2 Na1 O8 82.0(4) 1_655 1_655 ?
O2 Na1 O10 158.9(5) 1_655 . ?
O2 Na1 O13 115.1(5) 1_655 . ?
O2 Na1 O14 82.6(5) 1_655 2_666 ?
O7 Na1 U1 75.5(3) 2_667 1_655 ?
O7 Na1 U2 75.8(3) 2_667 1_655 ?
O7 Na1 U2 21.4(3) 2_667 2_667 ?
O7 Na1 U3 82.0(3) 2_667 . ?
O7 Na1 U4 127.3(4) 2_667 . ?
O7 Na1 U4 83.7(3) 2_667 2_666 ?
O7 Na1 O8 94.4(5) 2_667 1_655 ?
O7 Na1 O13 150.8(5) 2_667 . ?
O8 Na1 U1 72.3(3) 1_655 1_655 ?
O8 Na1 U2 21.1(3) 1_655 1_655 ?
O8 Na1 U2 76.2(3) 1_655 2_667 ?
O8 Na1 U3 103.3(3) 1_655 . ?
O8 Na1 U4 172.3(4) 1_655 2_666 ?
O8 Na1 U4 122.1(4) 1_655 . ?
O8 Na1 O13 104.7(4) 1_655 . ?
O10 Na1 U1 142.2(4) . 1_655 ?
O10 Na1 U2 87.1(4) . 1_655 ?
O10 Na1 U2 89.8(4) . 2_667 ?
O10 Na1 U3 23.6(3) . . ?
O10 Na1 U4 92.6(4) . 2_666 ?
O10 Na1 U4 70.4(3) . . ?
O10 Na1 O7 82.1(5) . 2_667 ?
O10 Na1 O8 79.8(4) . 1_655 ?
O10 Na1 O13 80.0(4) . . ?
O10 Na1 O14 114.3(5) . 2_666 ?
O13 Na1 U1 131.1(3) . 1_655 ?
O13 Na1 U2 169.4(4) . 2_667 ?
O13 Na1 U2 125.7(4) . 1_655 ?
O13 Na1 U3 72.4(3) . . ?
O13 Na1 U4 23.8(3) . . ?
O13 Na1 U4 74.3(3) . 2_666 ?
O14 Na1 U1 91.7(4) 2_666 1_655 ?
O14 Na1 U2 145.5(4) 2_666 1_655 ?
O14 Na1 U2 95.4(4) 2_666 2_667 ?
O14 Na1 U3 91.2(4) 2_666 . ?
O14 Na1 U4 71.9(4) 2_666 . ?
O14 Na1 U4 22.9(3) 2_666 2_666 ?
O14 Na1 O7 80.5(5) 2_666 2_667 ?
O14 Na1 O8 163.9(5) 2_666 1_655 ?
O14 Na1 O13 86.2(5) 2_666 . ?
U1 O2 Na1 138.5(7) . 1_455 ?
U1 O3 U1 110.7(5) . 2_557 ?
U1 O3 U2 137.6(5) . 1_545 ?
U2 O3 U1 99.4(4) 1_545 2_557 ?
U1 O4 U3 136.8(6) . 1_545 ?
U1 O5 U2 121.3(6) . . ?
U1 O5 U2 123.4(6) . 2_567 ?
U2 O5 U2 110.8(5) 2_567 . ?
U2 O6 U1 99.2(4) . . ?
U4 O6 U1 111.8(5) 2_666 . ?
U4 O6 U2 122.1(5) 2_666 . ?
U2 O7 Na1 128.3(6) . 2_667 ?
U2 O8 Na1 127.2(6) . 1_455 ?
U2 O9 U3 135.1(6) . . ?
U3 O10 Na1 124.1(6) . . ?
U3 O11 Mg1 160.3(7) . . ?
U3 O12 U3 111.2(5) . 2_676 ?
U4 O12 U3 134.8(6) . 2_676 ?
U4 O12 U3 112.9(5) . . ?
U4 O13 Na1 116.8(6) . . ?
U4 O14 Na1 125.4(7) . 2_666 ?
U3 O15 U4 106.4(5) 2_666 2_666 ?
U4 O15 U3 145.1(6) . 2_666 ?
U4 O15 U4 108.4(5) . 2_666 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
U1 U2 O7 Na1 38.5(7) 2_567 . . 2_667 ?
U1 U2 O7 Na1 -83.9(7) . . . 2_667 ?
U1 U2 O8 Na1 44.3(6) . . . 1_455 ?
U1 U2 O8 Na1 -77.8(6) 2_567 . . 1_455 ?
U2 U1 O2 Na1 22.5(8) 2_567 . . 1_455 ?
U2 U1 O2 Na1 -35.4(8) . . . 1_455 ?
U2 U2 O7 Na1 -22.3(7) 2_567 . . 2_667 ?
U2 U2 O8 Na1 -16.9(6) 2_567 . . 1_455 ?
U3 U3 O10 Na1 -116.7(7) 2_676 . . . ?
U3 U3 O11 Mg1 41(2) 2_676 . . . ?
U3 U4 O13 Na1 39.6(5) . . . . ?
U3 U4 O14 Na1 -113.0(7) . . . 2_666 ?
U4 U3 O10 Na1 -49.5(7) . . . . ?
U4 U3 O11 Mg1 -26(2) . . . . ?
U4 U4 O13 Na1 -32.0(5) 2_666 . . . ?
U4 U4 O14 Na1 -41.4(7) 2_666 . . 2_666 ?
Na1 U2 O7 Na1 -43.8(13) 1_455 . . 2_667 ?
Na1 U2 O8 Na1 -36.7(13) 2_667 . . 1_455 ?
Na1 U3 O11 Mg1 -82(2) . . . . ?
Na1 U4 O13 Na1 -75.9(9) 2_666 . . . ?
Na1 U4 O14 Na1 -72.8(10) . . . 2_666 ?
O3 U1 O2 Na1 58.7(10) 2_557 . . 1_455 ?
O3 U1 O2 Na1 127.1(9) . . . 1_455 ?
O3 U2 O7 Na1 79.1(8) 1_565 . . 2_667 ?
O3 U2 O8 Na1 -118.2(7) 1_565 . . 1_455 ?
O4 U1 O2 Na1 -141.8(9) . . . 1_455 ?
O4 U3 O10 Na1 141.5(7) 1_565 . . . ?
O4 U3 O11 Mg1 143(2) 1_565 . . . ?
O5 U1 O2 Na1 -5.9(9) . . . 1_455 ?
O5 U2 O7 Na1 -56.6(8) . . . 2_667 ?
O5 U2 O7 Na1 12.4(8) 2_567 . . 2_667 ?
O5 U2 O8 Na1 17.5(7) . . . 1_455 ?
O5 U2 O8 Na1 -51.7(7) 2_567 . . 1_455 ?
O6 U1 O2 Na1 -74.8(9) . . . 1_455 ?
O6 U2 O7 Na1 -124.9(8) . . . 2_667 ?
O6 U2 O8 Na1 85.6(7) . . . 1_455 ?
O6 U4 O13 Na1 -169.1(6) 2_666 . . . ?
O6 U4 O14 Na1 95.8(7) 2_666 . . 2_666 ?
O9 U2 O7 Na1 162.6(8) . . . 2_667 ?
O9 U2 O8 Na1 158.1(7) . . . 1_455 ?
O9 U3 O10 Na1 65.0(7) . . . . ?
O9 U3 O11 Mg1 -140(2) . . . . ?
O12 U3 O10 Na1 -150.7(7) 2_676 . . . ?
O12 U3 O10 Na1 -82.0(7) . . . . ?
O12 U3 O11 Mg1 75(2) 2_676 . . . ?
O12 U3 O11 Mg1 7(2) . . . . ?
O12 U4 O13 Na1 73.6(6) . . . . ?
O12 U4 O14 Na1 -146.9(7) . . . 2_666 ?
O15 U3 O10 Na1 -12.7(7) 2_666 . . . ?
O15 U3 O11 Mg1 -63(2) 2_666 . . . ?
O15 U4 O13 Na1 3.0(6) 2_666 . . . ?
O15 U4 O13 Na1 -68.6(6) . . . . ?
O15 U4 O14 Na1 -4.8(7) . . . 2_666 ?
O15 U4 O14 Na1 -76.3(7) 2_666 . . 2_666 ?

_olex2_submission_special_instructions 'No special instructions were received'

# start Validation Reply Form
_vrf_PLAT029_p1_a                
;
PROBLEM: _diffrn_measured_fraction_theta_full value Low .      0.909 Why?  
RESPONSE: The alert arises due to only one circle data collection on the 
MX2 beamline.
;
_vrf_PLAT975_p1_a                
;
PROBLEM: Check Calcd Resid. Dens.  0.98Ang From O2      .       2.19 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium.
;
_vrf_PLAT196_p1_a                
;
PROBLEM: No TEMP record and _measurement_temperature .NE.        293 Degree
RESPONSE: Data collection at 100K.
;
_vrf_PLAT911_p1_a                
;
PROBLEM: Missing FCF Refl Between Thmin & STh/L=    0.594        225 Report
RESPONSE: The alert arises due to only one circle data collection on the 
MX2 beamline.
;
_vrf_PLAT971_p1_a                
;
PROBLEM: Check Calcd Resid. Dens.  0.97Ang From O13             3.40 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium.
;
_vrf_PLAT972_p1_a                
;
PROBLEM: Check Calcd Resid. Dens.  1.08Ang From U3             -2.81 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium.
;
_vrf_PLAT973_p1_a                
;
PROBLEM: Check Calcd Positive Resid. Density on        U4       1.97 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium.
;
# end Validation Reply Form
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_p-1_a
_database_code_depnum_ccdc_archive 'CCDC 2289969'
loop_
_audit_author_name
_audit_author_address
'Yingjie Zhang'
;Australian Nuclear Science and Technology Organisation
Australia
;
_audit_update_record             
;
2023-08-22 deposited with the CCDC.	2023-11-09 downloaded from the CCDC.
;
_audit_creation_date             2023-06-28
_audit_creation_method           
;
Olex2 1.5
(compiled 2021.12.09 svn.r5202d8cf for OlexSys, GUI svn.r6439)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Mg Na2 O26 U6'
_chemical_formula_sum            'Mg Na2 O26 U6'
_chemical_formula_weight         1914.47
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   7.0150(14)
_cell_length_b                   12.067(2)
_cell_length_c                   13.411(3)
_cell_angle_alpha                91.22(3)
_cell_angle_beta                 100.49(3)
_cell_angle_gamma                90.36(3)
_cell_volume                     1116.0(4)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    3362
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      24.995
_cell_measurement_theta_min      1.545
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    43.558
_exptl_absorpt_correction_T_max  0.4342
_exptl_absorpt_correction_T_min  0.2161
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2012/1 (Bruker,2012) was used for absorption correction.
wR2(int) was 0.1310 before and 0.0743 after correction.
The Ratio of minimum to maximum transmission is 0.4977.
The λ/2 correction factor is 0.0015.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    5.697
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       needle
_exptl_crystal_F_000             1588
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.005
_exptl_crystal_size_min          0.005
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0598
_diffrn_reflns_av_unetI/netI     0.0784
_diffrn_reflns_Laue_measured_fraction_full 0.942
_diffrn_reflns_Laue_measured_fraction_max 0.942
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            13469
_diffrn_reflns_point_group_measured_fraction_full 0.942
_diffrn_reflns_point_group_measured_fraction_max 0.942
_diffrn_reflns_theta_full        24.995
_diffrn_reflns_theta_max         24.995
_diffrn_reflns_theta_min         1.545
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.942
_diffrn_measured_fraction_theta_max 0.942
_diffrn_radiation_type           
'silicon double crystal monochromated synchrotron'
_diffrn_source                   'Australian Synchrotron MX2'
_diffrn_measurement_device_type  'Eiger Detector'
_diffrn_measurement_method       'π  scans'
_diffrn_radiation_wavelength     0.71079
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                3362
_reflns_number_total             3694
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_data_collection       'BlueIce (McPhillips, et al., 2002)'
_computing_data_reduction        'XDS (Kabsch, 1993)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         5.436
_refine_diff_density_min         -3.966
_refine_diff_density_rms         0.492
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.076
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     304
_refine_ls_number_reflns         3694
_refine_ls_number_restraints     486
_refine_ls_R_factor_all          0.0429
_refine_ls_R_factor_gt           0.0401
_refine_ls_restrained_S_all      1.011
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0303P)²+4.3035P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1023
_refine_ls_wR_factor_ref         0.1068
_refine_special_details          ?
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(O3) = Uanis(O5) = Uanis(O4)
2. Rigid body (RIGU) restrains
 All non-hydrogen atoms
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 1.32498(7) 0.57537(3) 0.76302(4) 0.01671(15) Uani 1 1 d . . . . .
U2 U 0.85094(7) 0.39392(4) 0.76683(4) 0.01737(15) Uani 1 1 d . . . . .
U3 U 0.37365(7) 0.27269(4) 0.78770(4) 0.01670(15) Uani 1 1 d . . . . .
U4 U 0.82257(7) 0.07747(4) 0.81025(4) 0.02133(16) Uani 1 1 d . . . . .
U5 U 0.37810(7) -0.11787(4) 0.80030(4) 0.01827(16) Uani 1 1 d . . . . .
U6 U 0.14295(7) 0.24066(4) 0.21557(4) 0.01653(15) Uani 1 1 d . . . . .
Mg1 Mg 0.2395(7) 0.2221(4) 0.5026(4) 0.0256(10) Uani 1 1 d . . . . .
Na1 Na 0.2611(8) 0.4339(4) 1.0089(4) 0.0284(13) Uani 1 1 d . . . . .
Na2 Na 0.7548(7) 0.2828(4) 1.0063(4) 0.0230(11) Uani 1 1 d . . . . .
O1 O 1.3771(14) 0.5678(7) 0.9022(8) 0.025(2) Uani 1 1 d . . . . .
O2 O 1.2635(13) 0.5802(8) 0.6233(7) 0.023(2) Uani 1 1 d . . . . .
O3 O 1.5421(12) 0.7121(7) 0.7655(7) 0.0187(11) Uani 1 1 d . . . . .
O4 O 1.5349(12) 0.4389(7) 0.7563(7) 0.0187(11) Uani 1 1 d . . . . .
O5 O 1.1657(12) 0.4137(7) 0.7643(7) 0.0187(11) Uani 1 1 d . . . . .
O6 O 0.8989(13) 0.4318(7) 0.9036(7) 0.0204(19) Uani 1 1 d . . . . .
O7 O 0.8118(13) 0.3550(8) 0.6328(7) 0.025(2) Uani 1 1 d . . . . .
O8 O 0.8943(14) 0.5783(7) 0.7261(7) 0.024(2) Uani 1 1 d . . . . .
O9 O 1.0724(14) 0.2126(8) 0.8278(10) 0.042(3) Uani 1 1 d . . . . .
O10 O 0.6912(13) 0.2433(8) 0.8004(8) 0.028(2) Uani 1 1 d . . . . .
O11 O 0.8624(14) 0.0902(8) 0.9494(8) 0.030(2) Uani 1 1 d . . . . .
O12 O 0.7997(18) 0.0729(9) 0.6722(9) 0.039(3) Uani 1 1 d . . . . .
O13 O 0.6900(13) -0.0880(7) 0.8056(7) 0.024(2) Uani 1 1 d . . . . .
O14 O 0.4513(13) 0.0797(7) 0.8366(7) 0.0247(19) Uani 1 1 d . . . . .
O15 O 0.4384(13) -0.1375(8) 0.9367(8) 0.027(2) Uani 1 1 d . . . . .
O16 O 0.3112(13) -0.0913(7) 0.6655(7) 0.0201(19) Uani 1 1 d . . . . .
O17 O 0.0722(13) -0.0571(7) 0.8379(8) 0.028(2) Uani 1 1 d . . . . .
O18 O 0.4271(14) 0.3067(8) 0.9223(7) 0.027(2) Uani 1 1 d . . . . .
O19 O 0.3179(13) 0.2282(7) 0.6560(7) 0.0222(19) Uani 1 1 d . . . . .
O20 O 0.1654(13) 0.2025(7) 0.3494(7) 0.0208(18) Uani 1 1 d . . . . .
O21 O 0.1038(13) 0.2814(8) 0.0821(8) 0.027(2) Uani 1 1 d . . . . .
O22 O -0.1747(13) 0.2653(7) 0.2078(8) 0.024(2) Uani 1 1 d . . . . .
O23 O 0.1304(15) 0.3863(8) 0.4965(8) 0.034(2) Uani 1 1 d . . . . .
O24 O 0.5042(14) 0.2830(9) 0.4853(8) 0.034(2) Uani 1 1 d . . . . .
O25 O 0.3177(17) 0.0570(8) 0.5057(8) 0.039(3) Uani 1 1 d . . . . .
O26 O -0.0458(14) 0.1788(9) 0.5079(8) 0.034(2) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 U2 3.9788(13) . ?
U1 U3 3.6867(10) 1_655 ?
U1 U5 3.7321(10) 1_665 ?
U1 Na1 3.819(6) 2_767 ?
U1 Na1 3.842(5) 1_655 ?
U1 Na2 3.638(5) 2_767 ?
U1 O1 1.840(10) . ?
U1 O2 1.847(9) . ?
U1 O3 2.235(8) . ?
U1 O4 2.228(9) . ?
U1 O5 2.244(8) . ?
U1 O22 2.260(9) 2_666 ?
U2 U3 3.7049(11) . ?
U2 U3 3.9210(12) 1_655 ?
U2 U4 3.8842(10) . ?
U2 Na1 3.821(6) 2_667 ?
U2 Na2 3.677(5) . ?
U2 O4 2.266(8) 1_455 ?
U2 O5 2.226(8) . ?
U2 O6 1.851(9) . ?
U2 O7 1.819(9) . ?
U2 O8 2.333(9) . ?
U2 O9 2.743(11) . ?
U2 O10 2.226(9) . ?
U3 Mg1 3.802(5) . ?
U3 Na1 3.719(6) . ?
U3 Na2 3.589(5) . ?
U3 O4 2.379(8) 1_455 ?
U3 O5 2.238(9) 1_455 ?
U3 O9 2.386(9) 1_455 ?
U3 O10 2.234(9) . ?
U3 O14 2.470(9) . ?
U3 O18 1.813(10) . ?
U3 O19 1.808(9) . ?
U4 U5 3.8781(13) . ?
U4 U6 3.8603(10) 2_656 ?
U4 Na2 3.670(5) . ?
U4 O9 2.363(9) . ?
U4 O10 2.205(10) . ?
U4 O11 1.839(11) . ?
U4 O12 1.828(11) . ?
U4 O13 2.192(9) . ?
U4 O14 2.692(9) . ?
U4 O17 2.380(9) 1_655 ?
U5 U6 3.9035(12) 2_556 ?
U5 U6 3.7200(12) 2_656 ?
U5 Na2 3.555(5) 2_657 ?
U5 O3 2.436(9) 1_445 ?
U5 O13 2.203(9) . ?
U5 O14 2.455(8) . ?
U5 O15 1.822(10) . ?
U5 O16 1.819(9) . ?
U5 O17 2.407(9) . ?
U5 O22 2.262(8) 2_556 ?
U6 Mg1 3.797(5) . ?
U6 Na1 3.859(5) 1_554 ?
U6 Na2 3.584(5) 1_454 ?
U6 O3 2.246(8) 2_766 ?
U6 O8 2.337(8) 2_666 ?
U6 O13 2.231(9) 2_656 ?
U6 O17 2.683(9) 2_556 ?
U6 O20 1.842(9) . ?
U6 O21 1.839(10) . ?
U6 O22 2.234(9) . ?
Mg1 O19 2.029(10) . ?
Mg1 O20 2.034(10) . ?
Mg1 O23 2.127(10) . ?
Mg1 O24 2.047(10) . ?
Mg1 O25 2.069(11) . ?
Mg1 O26 2.079(11) . ?
Na1 Na1 3.752(10) 2_667 ?
Na1 Na2 3.431(7) 2_667 ?
Na1 O1 2.600(11) 2_767 ?
Na1 O1 2.414(11) 1_455 ?
Na1 O6 2.672(11) 1_455 ?
Na1 O6 2.384(10) 2_667 ?
Na1 O18 2.345(11) . ?
Na1 O21 2.452(10) 1_556 ?
Na2 O1 2.441(11) 2_767 ?
Na2 O6 2.596(10) . ?
Na2 O10 2.746(12) . ?
Na2 O11 2.590(11) . ?
Na2 O15 2.429(10) 2_657 ?
Na2 O18 2.391(11) . ?
Na2 O21 2.474(10) 1_656 ?
Na2 O22 2.670(12) 1_656 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
U3 U1 U2 61.39(3) 1_655 . ?
U3 U1 U5 164.64(2) 1_655 1_665 ?
U3 U1 Na1 80.39(8) 1_655 2_767 ?
U3 U1 Na1 59.17(8) 1_655 1_655 ?
U5 U1 U2 126.91(3) 1_665 . ?
U5 U1 Na1 111.47(8) 1_665 1_655 ?
U5 U1 Na1 84.28(8) 1_665 2_767 ?
Na1 U1 U2 118.50(8) 2_767 . ?
Na1 U1 U2 60.57(9) 1_655 . ?
Na1 U1 Na1 58.65(13) 2_767 1_655 ?
Na2 U1 U2 88.73(8) 2_767 . ?
Na2 U1 U3 113.58(9) 2_767 1_655 ?
Na2 U1 U5 57.66(9) 2_767 1_665 ?
Na2 U1 Na1 54.53(11) 2_767 1_655 ?
Na2 U1 Na1 63.54(12) 2_767 2_767 ?
O1 U1 U2 87.7(3) . . ?
O1 U1 U3 80.7(3) . 1_655 ?
O1 U1 U5 86.5(3) . 1_665 ?
O1 U1 Na1 37.1(3) . 2_767 ?
O1 U1 Na1 29.4(3) . 1_655 ?
O1 U1 Na2 37.2(3) . 2_767 ?
O1 U1 O2 177.8(4) . . ?
O1 U1 O3 91.7(4) . . ?
O1 U1 O4 88.6(4) . . ?
O1 U1 O5 86.4(4) . . ?
O1 U1 O22 84.2(4) . 2_666 ?
O2 U1 U2 90.1(3) . . ?
O2 U1 U3 98.4(3) . 1_655 ?
O2 U1 U5 94.6(3) . 1_665 ?
O2 U1 Na1 148.6(3) . 1_655 ?
O2 U1 Na1 144.9(3) . 2_767 ?
O2 U1 Na2 142.6(3) . 2_767 ?
O2 U1 O3 90.4(4) . . ?
O2 U1 O4 91.9(4) . . ?
O2 U1 O5 91.8(4) . . ?
O2 U1 O22 95.7(4) . 2_666 ?
O3 U1 U2 165.7(2) . . ?
O3 U1 U3 132.5(2) . 1_655 ?
O3 U1 U5 38.9(2) . 1_665 ?
O3 U1 Na1 67.0(2) . 2_767 ?
O3 U1 Na1 120.8(3) . 1_655 ?
O3 U1 Na2 82.2(2) . 2_767 ?
O3 U1 O5 167.1(3) . . ?
O3 U1 O22 73.2(3) . 2_666 ?
O4 U1 U2 99.0(2) . . ?
O4 U1 U3 38.3(2) . 1_655 ?
O4 U1 U5 133.5(2) . 1_665 ?
O4 U1 Na1 82.7(2) . 1_655 ?
O4 U1 Na1 65.3(2) . 2_767 ?
O4 U1 Na2 125.2(3) . 2_767 ?
O4 U1 O3 95.3(3) . . ?
O4 U1 O5 72.0(3) . . ?
O4 U1 O22 166.2(3) . 2_666 ?
O5 U1 U2 27.0(2) . . ?
O5 U1 U3 34.6(2) . 1_655 ?
O5 U1 U5 153.3(2) . 1_665 ?
O5 U1 Na1 104.9(2) . 2_767 ?
O5 U1 Na1 57.1(2) . 1_655 ?
O5 U1 Na2 103.4(2) . 2_767 ?
O5 U1 O22 119.1(3) . 2_666 ?
O22 U1 U2 92.5(2) 2_666 . ?
O22 U1 U3 150.1(2) 2_666 1_655 ?
O22 U1 U5 34.4(2) 2_666 1_665 ?
O22 U1 Na1 102.4(3) 2_666 2_767 ?
O22 U1 Na1 96.5(3) 2_666 1_655 ?
O22 U1 Na2 47.0(3) 2_666 2_767 ?
U3 U2 U3 133.80(2) . 1_655 ?
U3 U2 U4 62.07(3) . . ?
U3 U2 Na1 80.14(8) . 2_667 ?
U4 U2 U3 71.76(3) . 1_655 ?
Na1 U2 U3 117.96(9) 2_667 1_655 ?
Na1 U2 U4 112.31(8) 2_667 . ?
Na2 U2 U3 96.33(9) . 1_655 ?
Na2 U2 U3 58.18(8) . . ?
Na2 U2 U4 57.98(9) . . ?
Na2 U2 Na1 54.42(11) . 2_667 ?
O4 U2 U3 38.2(2) 1_455 . ?
O4 U2 U3 171.9(2) 1_455 1_655 ?
O4 U2 U4 100.2(2) 1_455 . ?
O4 U2 Na1 65.1(2) 1_455 2_667 ?
O4 U2 Na2 79.4(2) 1_455 . ?
O4 U2 O8 85.2(3) 1_455 . ?
O4 U2 O9 135.4(3) 1_455 . ?
O5 U2 U3 162.4(2) . . ?
O5 U2 U3 28.6(2) . 1_655 ?
O5 U2 U4 100.4(2) . . ?
O5 U2 Na1 107.8(2) . 2_667 ?
O5 U2 Na2 113.1(2) . . ?
O5 U2 O4 159.4(3) . 1_455 ?
O5 U2 O8 74.2(3) . . ?
O5 U2 O9 65.0(3) . . ?
O6 U2 U3 90.9(3) . 1_655 ?
O6 U2 U3 91.0(3) . . ?
O6 U2 U4 94.5(3) . . ?
O6 U2 Na1 29.3(3) . 2_667 ?
O6 U2 Na2 41.4(3) . . ?
O6 U2 O4 90.3(4) . 1_455 ?
O6 U2 O5 89.5(4) . . ?
O6 U2 O8 90.5(4) . . ?
O6 U2 O9 84.0(4) . . ?
O6 U2 O10 89.5(4) . . ?
O7 U2 U3 90.4(3) . . ?
O7 U2 U3 87.2(3) . 1_655 ?
O7 U2 U4 85.0(3) . . ?
O7 U2 Na1 152.4(3) . 2_667 ?
O7 U2 Na2 138.9(3) . . ?
O7 U2 O4 91.5(4) . 1_455 ?
O7 U2 O5 88.9(4) . . ?
O7 U2 O6 178.1(4) . . ?
O7 U2 O8 89.9(4) . . ?
O7 U2 O9 94.5(4) . . ?
O7 U2 O10 90.9(4) . . ?
O8 U2 U3 123.4(2) . . ?
O8 U2 U3 102.8(2) . 1_655 ?
O8 U2 U4 172.6(2) . . ?
O8 U2 Na1 74.5(2) . 2_667 ?
O8 U2 Na2 128.5(2) . . ?
O8 U2 O9 138.8(3) . . ?
O9 U2 U3 97.62(19) . . ?
O9 U2 U3 36.88(19) . 1_655 ?
O9 U2 U4 36.96(19) . . ?
O9 U2 Na1 112.3(3) . 2_667 ?
O9 U2 Na2 67.4(3) . . ?
O10 U2 U3 33.9(2) . . ?
O10 U2 U3 100.0(2) . 1_655 ?
O10 U2 U4 28.6(2) . . ?
O10 U2 Na1 95.1(3) . 2_667 ?
O10 U2 Na2 48.1(3) . . ?
O10 U2 O4 72.0(3) . 1_455 ?
O10 U2 O5 128.6(3) . . ?
O10 U2 O8 157.3(3) . . ?
O10 U2 O9 63.8(3) . . ?
U1 U3 U2 71.05(3) 1_455 . ?
U1 U3 Mg1 92.56(8) 1_455 . ?
U1 U3 Na1 62.49(8) 1_455 . ?
U2 U3 Mg1 92.26(8) . . ?
U2 U3 Na1 100.84(8) . . ?
Na1 U3 Mg1 145.27(11) . . ?
Na2 U3 U1 96.00(9) . 1_455 ?
Na2 U3 U2 60.53(8) . . ?
Na2 U3 Mg1 146.45(11) . . ?
Na2 U3 Na1 65.02(12) . . ?
O4 U3 U1 35.5(2) 1_455 1_455 ?
O4 U3 U2 36.0(2) 1_455 . ?
O4 U3 Mg1 88.7(2) 1_455 . ?
O4 U3 Na1 83.7(2) 1_455 . ?
O4 U3 Na2 80.0(2) 1_455 . ?
O4 U3 O9 139.9(3) 1_455 1_455 ?
O4 U3 O14 139.4(3) 1_455 . ?
O5 U3 U1 34.7(2) 1_455 1_455 ?
O5 U3 U2 105.3(2) 1_455 . ?
O5 U3 Mg1 85.9(2) 1_455 . ?
O5 U3 Na1 59.7(3) 1_455 . ?
O5 U3 Na2 118.3(2) 1_455 . ?
O5 U3 O4 69.3(3) 1_455 1_455 ?
O5 U3 O9 71.5(3) 1_455 1_455 ?
O5 U3 O14 150.8(3) 1_455 . ?
O9 U3 U1 104.5(2) 1_455 1_455 ?
O9 U3 U2 170.2(3) 1_455 . ?
O9 U3 Mg1 96.8(3) 1_455 . ?
O9 U3 Na1 69.4(3) 1_455 . ?
O9 U3 Na2 112.2(3) 1_455 . ?
O9 U3 O14 79.3(3) 1_455 . ?
O10 U3 U1 104.3(2) . 1_455 ?
O10 U3 U2 33.7(2) . . ?
O10 U3 Mg1 96.6(3) . . ?
O10 U3 Na1 112.2(3) . . ?
O10 U3 Na2 49.9(3) . . ?
O10 U3 O4 69.8(3) . 1_455 ?
O10 U3 O5 138.9(3) . 1_455 ?
O10 U3 O9 147.6(4) . 1_455 ?
O10 U3 O14 69.7(3) . . ?
O14 U3 U1 168.4(2) . 1_455 ?
O14 U3 U2 103.5(2) . . ?
O14 U3 Mg1 97.9(2) . . ?
O14 U3 Na1 109.8(2) . . ?
O14 U3 Na2 72.5(2) . . ?
O18 U3 U1 83.5(3) . 1_455 ?
O18 U3 U2 88.3(3) . . ?
O18 U3 Mg1 175.6(3) . . ?
O18 U3 Na1 30.5(3) . . ?
O18 U3 Na2 36.6(3) . . ?
O18 U3 O4 89.2(4) . 1_455 ?
O18 U3 O5 89.7(4) . 1_455 ?
O18 U3 O9 82.4(4) . 1_455 ?
O18 U3 O10 86.3(4) . . ?
O18 U3 O14 86.2(4) . . ?
O19 U3 U1 100.7(3) . 1_455 ?
O19 U3 U2 94.1(3) . . ?
O19 U3 Mg1 8.2(3) . . ?
O19 U3 Na1 151.5(3) . . ?
O19 U3 Na2 142.9(3) . . ?
O19 U3 O4 94.8(4) . 1_455 ?
O19 U3 O5 93.1(4) . 1_455 ?
O19 U3 O9 95.4(4) . 1_455 ?
O19 U3 O10 93.6(4) . . ?
O19 U3 O14 89.8(4) . . ?
O19 U3 O18 175.7(4) . . ?
U2 U4 U3 56.71(2) . . ?
U5 U4 U2 130.64(3) . . ?
U5 U4 U3 74.53(2) . . ?
U6 U4 U2 163.70(2) 2_656 . ?
U6 U4 U3 131.27(3) 2_656 . ?
U6 U4 U5 57.46(2) 2_656 . ?
Na2 U4 U2 58.18(9) . . ?
Na2 U4 U3 56.37(8) . . ?
Na2 U4 U5 102.36(8) . . ?
Na2 U4 U6 137.62(9) . 2_656 ?
O9 U4 U2 44.3(3) . . ?
O9 U4 U3 99.4(3) . . ?
O9 U4 U5 172.7(3) . . ?
O9 U4 U6 129.1(3) . 2_656 ?
O9 U4 Na2 70.6(3) . . ?
O9 U4 O14 134.1(3) . . ?
O9 U4 O17 86.8(3) . 1_655 ?
O10 U4 U2 28.9(2) . . ?
O10 U4 U3 28.3(2) . . ?
O10 U4 U5 102.8(2) . . ?
O10 U4 U6 158.8(2) . 2_656 ?
O10 U4 Na2 48.2(3) . . ?
O10 U4 O9 71.2(3) . . ?
O10 U4 O14 65.9(3) . . ?
O10 U4 O17 157.8(3) . 1_655 ?
O11 U4 U2 95.1(3) . . ?
O11 U4 U3 90.7(3) . . ?
O11 U4 U5 92.5(3) . . ?
O11 U4 U6 98.7(3) . 2_656 ?
O11 U4 Na2 41.3(3) . . ?
O11 U4 O9 83.4(4) . . ?
O11 U4 O10 89.4(4) . . ?
O11 U4 O13 94.0(4) . . ?
O11 U4 O14 80.7(4) . . ?
O11 U4 O17 85.0(4) . 1_655 ?
O12 U4 U2 81.6(3) . . ?
O12 U4 U3 90.3(4) . . ?
O12 U4 U5 92.2(4) . . ?
O12 U4 U6 84.1(3) . 2_656 ?
O12 U4 Na2 137.0(4) . . ?
O12 U4 O9 91.9(5) . . ?
O12 U4 O10 89.3(4) . . ?
O12 U4 O11 175.2(5) . . ?
O12 U4 O13 90.3(4) . . ?
O12 U4 O14 103.0(4) . . ?
O12 U4 O17 94.5(4) . 1_655 ?
O13 U4 U2 157.4(2) . . ?
O13 U4 U3 102.6(2) . . ?
O13 U4 U5 28.2(2) . . ?
O13 U4 U6 29.5(2) . 2_656 ?
O13 U4 Na2 120.7(3) . . ?
O13 U4 O9 157.8(4) . . ?
O13 U4 O10 130.9(3) . . ?
O13 U4 O14 66.4(3) . . ?
O13 U4 O17 71.0(3) . 1_655 ?
O14 U4 U2 94.82(18) . . ?
O14 U4 U3 38.59(18) . . ?
O14 U4 U5 38.85(18) . . ?
O14 U4 U6 95.89(18) . 2_656 ?
O14 U4 Na2 69.1(2) . . ?
O17 U4 U2 130.3(2) 1_655 . ?
O17 U4 U3 172.0(2) 1_655 . ?
O17 U4 U5 98.9(2) 1_655 . ?
O17 U4 U6 43.3(2) 1_655 2_656 ?
O17 U4 Na2 122.1(3) 1_655 . ?
O17 U4 O14 133.7(3) 1_655 . ?
U1 U5 U4 131.28(3) 1_445 . ?
U1 U5 U6 63.56(3) 1_445 2_556 ?
U4 U5 U6 164.838(19) . 2_556 ?
U6 U5 U1 70.33(3) 2_656 1_445 ?
U6 U5 U4 61.027(19) 2_656 . ?
U6 U5 U6 133.89(2) 2_656 2_556 ?
Na2 U5 U1 59.85(9) 2_657 1_445 ?
Na2 U5 U4 129.53(9) 2_657 . ?
Na2 U5 U6 99.81(9) 2_657 2_656 ?
Na2 U5 U6 57.22(9) 2_657 2_556 ?
O3 U5 U1 35.14(18) 1_445 1_445 ?
O3 U5 U4 96.20(18) 1_445 . ?
O3 U5 U6 98.42(18) 1_445 2_556 ?
O3 U5 U6 35.64(18) 1_445 2_656 ?
O3 U5 Na2 81.6(2) 1_445 2_657 ?
O3 U5 O14 139.5(3) 1_445 . ?
O13 U5 U1 103.5(2) . 1_445 ?
O13 U5 U4 28.0(2) . . ?
O13 U5 U6 167.1(2) . 2_556 ?
O13 U5 U6 33.2(2) . 2_656 ?
O13 U5 Na2 117.2(3) . 2_657 ?
O13 U5 O3 68.7(3) . 1_445 ?
O13 U5 O14 70.8(3) . . ?
O13 U5 O17 149.7(3) . . ?
O13 U5 O22 137.6(3) . 2_556 ?
O14 U5 U1 173.2(2) . 1_445 ?
O14 U5 U4 43.5(2) . . ?
O14 U5 U6 104.0(2) . 2_656 ?
O14 U5 U6 122.0(2) . 2_556 ?
O14 U5 Na2 118.8(2) . 2_657 ?
O15 U5 U1 89.0(3) . 1_445 ?
O15 U5 U4 91.1(3) . . ?
O15 U5 U6 87.1(3) . 2_656 ?
O15 U5 U6 92.4(3) . 2_556 ?
O15 U5 Na2 39.1(3) . 2_657 ?
O15 U5 O3 91.9(4) . 1_445 ?
O15 U5 O13 86.8(4) . . ?
O15 U5 O14 86.9(4) . . ?
O15 U5 O17 83.6(4) . . ?
O15 U5 O22 87.6(4) . 2_556 ?
O16 U5 U1 93.6(3) . 1_445 ?
O16 U5 U4 88.6(3) . . ?
O16 U5 U6 87.2(3) . 2_556 ?
O16 U5 U6 95.5(3) . 2_656 ?
O16 U5 Na2 141.7(3) . 2_657 ?
O16 U5 O3 91.3(4) . 1_445 ?
O16 U5 O13 94.3(4) . . ?
O16 U5 O14 90.7(4) . . ?
O16 U5 O15 176.9(4) . . ?
O16 U5 O17 93.9(4) . . ?
O16 U5 O22 93.5(4) . 2_556 ?
O17 U5 U1 105.0(2) . 1_445 ?
O17 U5 U4 123.4(2) . . ?
O17 U5 U6 169.7(2) . 2_656 ?
O17 U5 U6 42.6(2) . 2_556 ?
O17 U5 Na2 70.2(2) . 2_657 ?
O17 U5 O3 140.1(3) . 1_445 ?
O17 U5 O14 79.9(3) . . ?
O22 U5 U1 34.4(2) 2_556 1_445 ?
O22 U5 U4 165.6(2) 2_556 . ?
O22 U5 U6 29.5(2) 2_556 2_556 ?
O22 U5 U6 104.5(2) 2_556 2_656 ?
O22 U5 Na2 48.7(3) 2_556 2_657 ?
O22 U5 O3 69.5(3) 2_556 1_445 ?
O22 U5 O14 150.6(3) 2_556 . ?
O22 U5 O17 70.8(3) 2_556 . ?
U5 U6 U4 61.51(3) 2_656 2_656 ?
U5 U6 Mg1 91.66(8) 2_656 . ?
U5 U6 Na1 83.88(9) 2_656 1_554 ?
Mg1 U6 U4 90.42(8) . 2_656 ?
Mg1 U6 Na1 139.15(11) . 1_554 ?
Na1 U6 U4 121.61(8) 1_554 2_656 ?
Na2 U6 U4 98.21(9) 1_454 2_656 ?
Na2 U6 U5 125.88(9) 1_454 2_656 ?
Na2 U6 Mg1 140.96(11) 1_454 . ?
Na2 U6 Na1 64.46(12) 1_454 1_554 ?
O3 U6 U4 100.2(2) 2_766 2_656 ?
O3 U6 U5 39.2(2) 2_766 2_656 ?
O3 U6 Mg1 85.1(2) 2_766 . ?
O3 U6 Na1 66.1(2) 2_766 1_554 ?
O3 U6 Na2 129.8(2) 2_766 1_454 ?
O3 U6 O8 84.4(3) 2_766 2_666 ?
O3 U6 O17 136.4(3) 2_766 2_556 ?
O8 U6 U4 164.7(2) 2_666 2_656 ?
O8 U6 U5 123.4(2) 2_666 2_656 ?
O8 U6 Mg1 75.3(2) 2_666 . ?
O8 U6 Na1 73.6(2) 2_666 1_554 ?
O8 U6 Na2 89.7(3) 2_666 1_454 ?
O8 U6 O17 139.1(3) 2_666 2_556 ?
O13 U6 U4 28.9(2) 2_656 2_656 ?
O13 U6 U5 32.7(2) 2_656 2_656 ?
O13 U6 Mg1 93.5(3) 2_656 . ?
O13 U6 Na1 103.5(3) 2_656 1_554 ?
O13 U6 Na2 112.1(3) 2_656 1_454 ?
O13 U6 O3 71.8(3) 2_656 2_766 ?
O13 U6 O8 154.6(3) 2_656 2_666 ?
O13 U6 O17 64.8(3) 2_656 2_556 ?
O13 U6 O22 130.8(3) 2_656 . ?
O17 U6 U4 37.49(19) 2_556 2_656 ?
O17 U6 U5 97.23(19) 2_556 2_656 ?
O17 U6 Mg1 101.1(2) 2_556 . ?
O17 U6 Na1 119.8(2) 2_556 1_554 ?
O17 U6 Na2 67.3(2) 2_556 1_454 ?
O20 U6 U4 79.8(3) . 2_656 ?
O20 U6 U5 91.6(3) . 2_656 ?
O20 U6 Mg1 12.2(3) . . ?
O20 U6 Na1 151.2(3) . 1_554 ?
O20 U6 Na2 136.5(3) . 1_454 ?
O20 U6 O3 92.8(4) . 2_766 ?
O20 U6 O8 85.5(4) . 2_666 ?
O20 U6 O13 86.9(4) . 2_656 ?
O20 U6 O17 89.0(3) . 2_556 ?
O20 U6 O22 89.5(4) . . ?
O21 U6 U4 101.6(3) . 2_656 ?
O21 U6 U5 92.1(3) . 2_656 ?
O21 U6 Mg1 167.8(3) . . ?
O21 U6 Na1 30.2(3) . 1_554 ?
O21 U6 Na2 39.9(3) . 1_454 ?
O21 U6 O3 90.5(4) . 2_766 ?
O21 U6 O8 92.9(4) . 2_666 ?
O21 U6 O13 96.0(4) . 2_656 ?
O21 U6 O17 90.0(4) . 2_556 ?
O21 U6 O20 176.2(4) . . ?
O21 U6 O22 86.7(4) . . ?
O22 U6 U4 102.3(2) . 2_656 ?
O22 U6 U5 163.2(2) . 2_656 ?
O22 U6 Mg1 92.9(3) . . ?
O22 U6 Na1 102.9(3) . 1_554 ?
O22 U6 Na2 48.0(3) . 1_454 ?
O22 U6 O3 157.4(3) . 2_766 ?
O22 U6 O8 73.4(3) . 2_666 ?
O22 U6 O17 66.1(3) . 2_556 ?
U6 Mg1 U3 166.75(14) . . ?
O19 Mg1 U3 7.3(3) . . ?
O19 Mg1 U6 172.4(3) . . ?
O19 Mg1 O20 175.3(5) . . ?
O19 Mg1 O23 93.2(4) . . ?
O19 Mg1 O24 91.5(4) . . ?
O19 Mg1 O25 88.3(4) . . ?
O19 Mg1 O26 93.1(4) . . ?
O20 Mg1 U3 177.4(3) . . ?
O20 Mg1 U6 11.0(2) . . ?
O20 Mg1 O23 91.4(4) . . ?
O20 Mg1 O24 89.3(4) . . ?
O20 Mg1 O25 87.0(4) . . ?
O20 Mg1 O26 86.6(4) . . ?
O23 Mg1 U3 86.1(3) . . ?
O23 Mg1 U6 83.6(3) . . ?
O24 Mg1 U3 90.1(3) . . ?
O24 Mg1 U6 81.6(3) . . ?
O24 Mg1 O23 89.5(5) . . ?
O24 Mg1 O25 95.9(5) . . ?
O24 Mg1 O26 171.9(5) . . ?
O25 Mg1 U3 95.5(3) . . ?
O25 Mg1 U6 95.6(3) . . ?
O25 Mg1 O23 174.4(5) . . ?
O25 Mg1 O26 90.9(5) . . ?
O26 Mg1 U3 93.6(3) . . ?
O26 Mg1 U6 93.4(3) . . ?
O26 Mg1 O23 83.7(5) . . ?
U1 Na1 U1 121.35(13) 2_767 1_455 ?
U1 Na1 U2 68.42(10) 2_767 2_667 ?
U2 Na1 U1 120.27(13) 2_667 1_455 ?
U3 Na1 U1 58.34(8) . 1_455 ?
U3 Na1 U1 111.83(14) . 2_767 ?
U3 Na1 U2 178.56(15) . 2_667 ?
U3 Na1 Na1 80.85(17) . 2_667 ?
Na1 Na1 U1 60.98(16) 2_667 2_767 ?
Na1 Na1 U1 60.36(14) 2_667 1_455 ?
Na1 Na1 U2 98.2(2) 2_667 2_667 ?
Na2 Na1 U1 59.71(13) 2_667 1_455 ?
Na2 Na1 U1 96.32(16) 2_667 2_767 ?
Na2 Na1 U2 60.66(13) 2_667 2_667 ?
Na2 Na1 U3 117.93(19) 2_667 . ?
Na2 Na1 Na1 66.15(17) 2_667 2_667 ?
O1 Na1 U1 25.3(2) 2_767 2_767 ?
O1 Na1 U1 102.7(3) 1_455 2_767 ?
O1 Na1 U1 98.5(3) 2_767 1_455 ?
O1 Na1 U1 22.0(2) 1_455 1_455 ?
O1 Na1 U2 104.3(3) 1_455 2_667 ?
O1 Na1 U2 88.6(3) 2_767 2_667 ?
O1 Na1 U3 91.3(3) 2_767 . ?
O1 Na1 U3 74.3(3) 1_455 . ?
O1 Na1 Na1 43.5(3) 1_455 2_667 ?
O1 Na1 Na1 39.7(2) 2_767 2_667 ?
O1 Na1 Na2 45.3(3) 1_455 2_667 ?
O1 Na1 Na2 94.0(3) 2_767 2_667 ?
O1 Na1 O1 83.2(4) 1_455 2_767 ?
O1 Na1 O6 175.4(4) 2_767 1_455 ?
O1 Na1 O6 94.1(4) 1_455 1_455 ?
O1 Na1 O21 167.5(4) 1_455 1_556 ?
O6 Na1 U1 89.9(3) 2_667 2_767 ?
O6 Na1 U1 78.0(2) 1_455 1_455 ?
O6 Na1 U1 159.1(3) 1_455 2_767 ?
O6 Na1 U1 104.5(3) 2_667 1_455 ?
O6 Na1 U2 95.7(2) 1_455 2_667 ?
O6 Na1 U2 22.3(2) 2_667 2_667 ?
O6 Na1 U3 157.0(3) 2_667 . ?
O6 Na1 U3 84.4(2) 1_455 . ?
O6 Na1 Na1 104.7(3) 2_667 2_667 ?
O6 Na1 Na1 137.5(3) 1_455 2_667 ?
O6 Na1 Na2 49.1(2) 2_667 2_667 ?
O6 Na1 Na2 86.7(3) 1_455 2_667 ?
O6 Na1 O1 94.3(4) 2_667 1_455 ?
O6 Na1 O1 107.3(4) 2_667 2_767 ?
O6 Na1 O6 76.5(4) 2_667 1_455 ?
O6 Na1 O21 91.4(4) 2_667 1_556 ?
O18 Na1 U1 89.4(3) . 2_767 ?
O18 Na1 U1 74.2(3) . 1_455 ?
O18 Na1 U2 157.5(3) . 2_667 ?
O18 Na1 U3 23.1(2) . . ?
O18 Na1 Na1 73.2(3) . 2_667 ?
O18 Na1 Na2 129.1(3) . 2_667 ?
O18 Na1 O1 71.4(3) . 2_767 ?
O18 Na1 O1 84.0(4) . 1_455 ?
O18 Na1 O6 177.9(4) . 2_667 ?
O18 Na1 O6 104.7(4) . 1_455 ?
O18 Na1 O21 90.6(4) . 1_556 ?
O21 Na1 U1 145.5(3) 1_556 1_455 ?
O21 Na1 U1 88.5(3) 1_556 2_767 ?
O21 Na1 U2 85.0(3) 1_556 2_667 ?
O21 Na1 U3 96.4(3) 1_556 . ?
O21 Na1 Na1 144.7(4) 1_556 2_667 ?
O21 Na1 Na2 140.0(3) 1_556 2_667 ?
O21 Na1 O1 105.8(4) 1_556 2_767 ?
O21 Na1 O6 76.3(3) 1_556 1_455 ?
U5 Na2 U3 109.48(13) 2_657 . ?
U5 Na2 U6 66.29(10) 2_657 1_656 ?
U6 Na2 U3 169.71(17) 1_656 . ?
Na1 Na2 U3 87.25(16) 2_667 . ?
Na1 Na2 U5 127.28(19) 2_667 2_657 ?
Na1 Na2 U6 102.78(17) 2_667 1_656 ?
O1 Na2 U3 97.2(3) 2_767 . ?
O1 Na2 U5 83.0(3) 2_767 2_657 ?
O1 Na2 U6 91.7(3) 2_767 1_656 ?
O1 Na2 Na1 44.7(3) 2_767 2_667 ?
O1 Na2 O6 88.5(3) 2_767 . ?
O1 Na2 O10 127.5(4) 2_767 . ?
O1 Na2 O11 163.3(4) 2_767 . ?
O1 Na2 O21 104.3(4) 2_767 1_656 ?
O1 Na2 O22 65.3(3) 2_767 1_656 ?
O6 Na2 U3 83.1(2) . . ?
O6 Na2 U5 165.6(3) . 2_657 ?
O6 Na2 U6 102.5(3) . 1_656 ?
O6 Na2 Na1 43.9(2) . 2_667 ?
O6 Na2 O10 65.2(3) . . ?
O6 Na2 O22 126.1(3) . 1_656 ?
O10 Na2 U3 38.5(2) . . ?
O10 Na2 U5 129.1(2) . 2_657 ?
O10 Na2 U6 136.4(3) . 1_656 ?
O10 Na2 Na1 95.4(3) . 2_667 ?
O11 Na2 U3 87.9(3) . . ?
O11 Na2 U5 80.3(3) . 2_657 ?
O11 Na2 U6 82.2(3) . 1_656 ?
O11 Na2 Na1 151.9(3) . 2_667 ?
O11 Na2 O6 107.9(4) . . ?
O11 Na2 O10 64.7(3) . . ?
O11 Na2 O22 101.4(4) . 1_656 ?
O15 Na2 U3 82.7(3) 2_657 . ?
O15 Na2 U5 28.2(2) 2_657 2_657 ?
O15 Na2 U6 91.3(3) 2_657 1_656 ?
O15 Na2 Na1 136.7(3) 2_657 2_667 ?
O15 Na2 O1 95.0(4) 2_657 2_767 ?
O15 Na2 O6 165.7(4) 2_657 . ?
O15 Na2 O10 102.1(4) 2_657 . ?
O15 Na2 O11 69.8(3) 2_657 . ?
O15 Na2 O21 115.0(4) 2_657 1_656 ?
O15 Na2 O22 67.6(3) 2_657 1_656 ?
O18 Na2 U3 26.8(2) . . ?
O18 Na2 U5 93.7(3) . 2_657 ?
O18 Na2 U6 156.8(3) . 1_656 ?
O18 Na2 Na1 79.5(3) . 2_667 ?
O18 Na2 O1 73.6(4) . 2_767 ?
O18 Na2 O6 95.1(4) . . ?
O18 Na2 O10 65.2(3) . . ?
O18 Na2 O11 106.9(4) . . ?
O18 Na2 O15 72.8(4) . 2_657 ?
O18 Na2 O21 172.2(4) . 1_656 ?
O18 Na2 O22 118.4(4) . 1_656 ?
O21 Na2 U3 150.4(3) 1_656 . ?
O21 Na2 U5 93.4(3) 1_656 2_657 ?
O21 Na2 U6 28.5(2) 1_656 1_656 ?
O21 Na2 Na1 93.7(3) 1_656 2_667 ?
O21 Na2 O6 77.4(3) 1_656 . ?
O21 Na2 O10 112.2(4) 1_656 . ?
O21 Na2 O11 77.4(3) 1_656 . ?
O21 Na2 O22 66.1(3) 1_656 1_656 ?
O22 Na2 U3 142.9(3) 1_656 . ?
O22 Na2 U5 39.5(2) 1_656 2_657 ?
O22 Na2 U6 38.5(2) 1_656 1_656 ?
O22 Na2 Na1 99.2(3) 1_656 2_667 ?
O22 Na2 O10 165.4(3) 1_656 . ?
U1 O1 Na1 117.6(5) . 2_767 ?
U1 O1 Na1 128.6(5) . 1_655 ?
U1 O1 Na2 115.7(5) . 2_767 ?
Na1 O1 Na1 96.8(4) 1_655 2_767 ?
Na1 O1 Na2 89.9(4) 1_655 2_767 ?
Na2 O1 Na1 102.4(4) 2_767 2_767 ?
U1 O3 U5 106.0(3) . 1_665 ?
U1 O3 U6 146.7(4) . 2_766 ?
U6 O3 U5 105.2(3) 2_766 1_665 ?
U1 O4 U2 145.8(4) . 1_655 ?
U1 O4 U3 106.3(3) . 1_655 ?
U2 O4 U3 105.8(3) 1_655 1_655 ?
U2 O5 U1 125.8(4) . . ?
U2 O5 U3 122.9(4) . 1_655 ?
U3 O5 U1 110.7(3) 1_655 . ?
U2 O6 Na1 120.3(4) . 1_655 ?
U2 O6 Na1 128.4(5) . 2_667 ?
U2 O6 Na2 110.4(4) . . ?
Na1 O6 Na1 103.5(4) 2_667 1_655 ?
Na1 O6 Na2 87.0(3) 2_667 . ?
Na2 O6 Na1 98.0(3) . 1_655 ?
U2 O8 U6 141.6(4) . 2_666 ?
U3 O9 U2 99.5(3) 1_655 . ?
U4 O9 U2 98.8(4) . . ?
U4 O9 U3 148.9(5) . 1_655 ?
U2 O10 U3 112.4(4) . . ?
U2 O10 Na2 94.8(4) . . ?
U3 O10 Na2 91.6(4) . . ?
U4 O10 U2 122.5(4) . . ?
U4 O10 U3 123.8(4) . . ?
U4 O10 Na2 95.0(4) . . ?
U4 O11 Na2 110.8(5) . . ?
U4 O13 U5 123.9(4) . . ?
U4 O13 U6 121.6(4) . 2_656 ?
U5 O13 U6 114.1(4) . 2_656 ?
U3 O14 U4 98.6(3) . . ?
U5 O14 U3 146.8(4) . . ?
U5 O14 U4 97.7(3) . . ?
U5 O15 Na2 112.7(4) . 2_657 ?
U4 O17 U5 146.8(4) 1_455 . ?
U4 O17 U6 99.2(3) 1_455 2_556 ?
U5 O17 U6 100.0(3) . 2_556 ?
U3 O18 Na1 126.4(5) . . ?
U3 O18 Na2 116.6(5) . . ?
Na1 O18 Na2 112.1(4) . . ?
U3 O19 Mg1 164.6(5) . . ?
U6 O20 Mg1 156.9(5) . . ?
U6 O21 Na1 127.6(5) . 1_554 ?
U6 O21 Na2 111.5(4) . 1_454 ?
Na1 O21 Na2 107.6(4) 1_554 1_454 ?
U1 O22 U5 111.3(4) 2_666 2_556 ?
U1 O22 Na2 94.8(4) 2_666 1_454 ?
U5 O22 Na2 91.8(3) 2_556 1_454 ?
U6 O22 U1 127.2(4) . 2_666 ?
U6 O22 U5 120.5(4) . 2_556 ?
U6 O22 Na2 93.5(4) . 1_454 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
U1 U3 O18 Na1 43.8(5) 1_455 . . . ?
U1 U3 O18 Na2 -109.4(4) 1_455 . . . ?
U1 U3 O19 Mg1 -6(2) 1_455 . . . ?
U1 U5 O15 Na2 -39.1(4) 1_445 . . 2_657 ?
U2 U1 O1 Na1 147.7(4) . . . 2_767 ?
U2 U1 O1 Na1 21.6(6) . . . 1_655 ?
U2 U1 O1 Na2 -91.0(4) . . . 2_767 ?
U2 U3 O18 Na1 115.0(5) . . . . ?
U2 U3 O18 Na2 -38.2(4) . . . . ?
U2 U3 O19 Mg1 -77(2) . . . . ?
U2 U4 O11 Na2 25.3(4) . . . . ?
U3 U1 O1 Na1 86.3(4) 1_655 . . 2_767 ?
U3 U1 O1 Na1 -39.8(5) 1_655 . . 1_655 ?
U3 U1 O1 Na2 -152.3(5) 1_655 . . 2_767 ?
U3 U2 O6 Na1 14.4(4) 1_655 . . 1_655 ?
U3 U2 O6 Na1 148.3(4) . . . 1_655 ?
U3 U2 O6 Na1 158.5(5) 1_655 . . 2_667 ?
U3 U2 O6 Na1 -67.6(5) . . . 2_667 ?
U3 U2 O6 Na2 35.3(3) . . . . ?
U3 U2 O6 Na2 -98.5(3) 1_655 . . . ?
U3 U4 O11 Na2 -31.4(4) . . . . ?
U4 U2 O6 Na1 -129.7(5) . . . 2_667 ?
U4 U2 O6 Na1 86.2(4) . . . 1_655 ?
U4 U2 O6 Na2 -26.8(4) . . . . ?
U4 U5 O15 Na2 -170.4(4) . . . 2_657 ?
U4 U6 O20 Mg1 150.9(14) 2_656 . . . ?
U4 U6 O21 Na1 -135.3(5) 2_656 . . 1_554 ?
U4 U6 O21 Na2 89.0(4) 2_656 . . 1_454 ?
U5 U1 O1 Na1 -85.1(4) 1_665 . . 2_767 ?
U5 U1 O1 Na1 148.8(6) 1_665 . . 1_655 ?
U5 U1 O1 Na2 36.2(4) 1_665 . . 2_767 ?
U5 U4 O11 Na2 -105.9(4) . . . . ?
U5 U6 O20 Mg1 90.3(14) 2_656 . . . ?
U5 U6 O21 Na1 -74.0(5) 2_656 . . 1_554 ?
U5 U6 O21 Na2 150.3(4) 2_656 . . 1_454 ?
U6 U4 O11 Na2 -163.4(3) 2_656 . . . ?
U6 U5 O15 Na2 -109.5(4) 2_656 . . 2_657 ?
U6 U5 O15 Na2 24.4(4) 2_556 . . 2_657 ?
Mg1 U6 O21 Na1 34.0(18) . . . 1_554 ?
Mg1 U6 O21 Na2 -101.6(13) . . . 1_454 ?
Na1 U1 O1 Na1 -126.1(8) 2_767 . . 1_655 ?
Na1 U1 O1 Na1 126.1(8) 1_655 . . 2_767 ?
Na1 U1 O1 Na2 121.3(7) 2_767 . . 2_767 ?
Na1 U1 O1 Na2 -112.5(8) 1_655 . . 2_767 ?
Na1 U2 O6 Na1 -144.1(8) 2_667 . . 1_655 ?
Na1 U2 O6 Na2 103.0(7) 2_667 . . . ?
Na1 U3 O18 Na2 -153.2(9) . . . . ?
Na1 U3 O19 Mg1 44(2) . . . . ?
Na1 U6 O20 Mg1 10.0(19) 1_554 . . . ?
Na1 U6 O21 Na2 -135.7(9) 1_554 . . 1_454 ?
Na2 U1 O1 Na1 -121.3(7) 2_767 . . 2_767 ?
Na2 U1 O1 Na1 112.5(8) 2_767 . . 1_655 ?
Na2 U2 O6 Na1 -103.0(7) . . . 2_667 ?
Na2 U2 O6 Na1 113.0(6) . . . 1_655 ?
Na2 U3 O18 Na1 153.2(9) . . . . ?
Na2 U3 O19 Mg1 -121.1(19) . . . . ?
Na2 U6 O20 Mg1 -117.9(13) 1_454 . . . ?
Na2 U6 O21 Na1 135.7(9) 1_454 . . 1_554 ?
O3 U1 O1 Na1 -46.6(4) . . . 2_767 ?
O3 U1 O1 Na1 -172.7(6) . . . 1_655 ?
O3 U1 O1 Na2 74.8(5) . . . 2_767 ?
O3 U5 O15 Na2 -74.1(4) 1_445 . . 2_657 ?
O3 U6 O20 Mg1 51.1(14) 2_766 . . . ?
O3 U6 O21 Na1 -34.8(6) 2_766 . . 1_554 ?
O3 U6 O21 Na2 -170.5(4) 2_766 . . 1_454 ?
O4 U1 O1 Na1 48.7(4) . . . 2_767 ?
O4 U1 O1 Na1 -77.5(6) . . . 1_655 ?
O4 U1 O1 Na2 170.0(5) . . . 2_767 ?
O4 U2 O6 Na1 -173.6(4) 1_455 . . 1_655 ?
O4 U2 O6 Na1 -29.5(5) 1_455 . . 2_667 ?
O4 U2 O6 Na2 73.5(4) 1_455 . . . ?
O4 U3 O18 Na1 78.9(6) 1_455 . . . ?
O4 U3 O18 Na2 -74.3(5) 1_455 . . . ?
O4 U3 O19 Mg1 -41(2) 1_455 . . . ?
O5 U1 O1 Na1 -5.4(6) . . . 1_655 ?
O5 U1 O1 Na1 120.7(4) . . . 2_767 ?
O5 U1 O1 Na2 -118.0(5) . . . 2_767 ?
O5 U2 O6 Na1 129.9(5) . . . 2_667 ?
O5 U2 O6 Na1 -14.2(5) . . . 1_655 ?
O5 U2 O6 Na2 -127.1(4) . . . . ?
O5 U3 O18 Na1 9.6(6) 1_455 . . . ?
O5 U3 O18 Na2 -143.6(5) 1_455 . . . ?
O5 U3 O19 Mg1 28(2) 1_455 . . . ?
O8 U2 O6 Na1 -88.3(5) . . . 1_655 ?
O8 U2 O6 Na1 55.7(5) . . . 2_667 ?
O8 U2 O6 Na2 158.7(4) . . . . ?
O8 U6 O20 Mg1 -33.1(14) 2_666 . . . ?
O8 U6 O21 Na1 49.6(6) 2_666 . . 1_554 ?
O8 U6 O21 Na2 -86.1(4) 2_666 . . 1_454 ?
O9 U2 O6 Na1 50.7(4) . . . 1_655 ?
O9 U2 O6 Na1 -165.2(6) . . . 2_667 ?
O9 U2 O6 Na2 -62.2(4) . . . . ?
O9 U3 O18 Na1 -61.8(6) 1_455 . . . ?
O9 U3 O18 Na2 145.0(5) 1_455 . . . ?
O9 U3 O19 Mg1 100(2) 1_455 . . . ?
O9 U4 O11 Na2 68.0(4) . . . . ?
O10 U2 O6 Na1 -101.5(6) . . . 2_667 ?
O10 U2 O6 Na1 114.4(5) . . . 1_655 ?
O10 U2 O6 Na2 1.4(4) . . . . ?
O10 U3 O18 Na1 148.7(6) . . . . ?
O10 U3 O18 Na2 -4.5(5) . . . . ?
O10 U3 O19 Mg1 -111(2) . . . . ?
O10 U4 O11 Na2 -3.1(4) . . . . ?
O13 U4 O11 Na2 -134.1(4) . . . . ?
O13 U5 O15 Na2 -142.7(5) . . . 2_657 ?
O13 U6 O20 Mg1 122.7(14) 2_656 . . . ?
O13 U6 O21 Na1 -106.6(6) 2_656 . . 1_554 ?
O13 U6 O21 Na2 117.7(4) 2_656 . . 1_454 ?
O14 U3 O18 Na1 -141.4(6) . . . . ?
O14 U3 O18 Na2 65.4(5) . . . . ?
O14 U3 O19 Mg1 179(2) . . . . ?
O14 U4 O11 Na2 -68.8(4) . . . . ?
O14 U5 O15 Na2 146.3(5) . . . 2_657 ?
O17 U4 O11 Na2 155.4(4) 1_655 . . . ?
O17 U5 O15 Na2 66.1(4) . . . 2_657 ?
O17 U6 O20 Mg1 -172.5(14) 2_556 . . . ?
O17 U6 O21 Na1 -171.2(6) 2_556 . . 1_554 ?
O17 U6 O21 Na2 53.1(4) 2_556 . . 1_454 ?
O22 U1 O1 Na1 -119.5(5) 2_666 . . 2_767 ?
O22 U1 O1 Na1 114.3(6) 2_666 . . 1_655 ?
O22 U1 O1 Na2 1.8(4) 2_666 . . 2_767 ?
O22 U5 O15 Na2 -4.8(5) 2_556 . . 2_657 ?
O22 U6 O20 Mg1 -106.5(14) . . . . ?
O22 U6 O21 Na1 122.7(6) . . . 1_554 ?
O22 U6 O21 Na2 -12.9(4) . . . 1_454 ?

_olex2_submission_special_instructions 'No special instructions were received'

# start Validation Reply Form
_vrf_PLAT971_p-1_a               
;
PROBLEM: Check Calcd Resid. Dens.  0.82Ang From U4              4.05 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium and 
ineffective absorption corrections.
;
_vrf_PLAT972_p-1_a               
;
PROBLEM: Check Calcd Resid. Dens.  0.78Ang From U4             -4.13 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium and 
ineffective absorption corrections.
;
_vrf_PLAT973_p-1_a               
;
PROBLEM: Check Calcd Positive Resid. Density on        U3       5.85 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium and 
ineffective absorption corrections.
;
_vrf_PLAT975_p-1_a               
;
PROBLEM: Check Calcd Resid. Dens.  1.08Ang From O8      .       2.47 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium and 
ineffective absorption corrections.
;
_vrf_PLAT029_p-1_a               
;
PROBLEM: _diffrn_measured_fraction_theta_full value Low .      0.942 Why?  
RESPONSE: The alert arises due to only one circle data collection possible 
on the MX2 beam.
;
_vrf_PLAT196_p-1_a               
;
PROBLEM: No TEMP record and _measurement_temperature .NE.        293 Degree
RESPONSE: The alert arises due to data collection at 100K.
;
_vrf_PLAT911_p-1_a               
;
PROBLEM: Missing FCF Refl Between Thmin & STh/L=    0.594        228 Report
RESPONSE: The alert arises due to only one circle data collection possible 
on the MX2 beam.
;
_vrf_PLAT976_p-1_a               
;
PROBLEM: Check Calcd Resid. Dens.  0.90Ang From O1      .      -1.51 eA-3  
RESPONSE: he alert arises due to strong absorption of uranium and 
ineffective absorption corrections.
;
# end Validation Reply Form
